#------------------------------------------------------------------------------
#$Date: 2019-11-23 08:34:00 +0200 (Sat, 23 Nov 2019) $
#$Revision: 232569 $
#$URL: file:///home/coder/svn-repositories/cod/cif/4/34/78/4347890.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4347890
loop_
_publ_author_name
'Li, Lei-Lei'
'Cao, Gao-Juan'
'Zhao, Jun-Wei'
'He, Huan'
'Yang, Bai-Feng'
'Yang, Guo-Yu'
_publ_section_title
;
 Lanthanide Germanate Cluster Organic Frameworks Based on {Ln8Ge12}
 Clusters: From One-Dimensional Chains to Two-Dimensional Layers and
 Three-Dimensional Frameworks.
;
_journal_issue                   11
_journal_name_full               'Inorganic chemistry'
_journal_page_first              5671
_journal_page_last               5683
_journal_paper_doi               10.1021/acs.inorgchem.6b00754
_journal_volume                  55
_journal_year                    2016
_chemical_formula_moiety         '0.5(C108 H168 Ge28 N4 O144 Tb20), 10(O)'
_chemical_formula_sum            'C54 H108 Ge14 N2 O82 Tb10'
_chemical_formula_weight         4702.88
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2ybc'
_space_group_name_H-M_alt        'P 1 21/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_date             2016-05-04
_audit_creation_method
;
Olex2 1.2
(compiled 2016.02.19 svn.r3266 for OlexSys, GUI svn.r5155)
;
_cell_angle_alpha                90.00
_cell_angle_beta                 115.926(4)
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   17.660(5)
_cell_length_b                   20.309(5)
_cell_length_c                   17.565(5)
_cell_measurement_reflns_used    12158
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      27.4603
_cell_measurement_theta_min      3.0598
_cell_volume                     5666(3)
_computing_cell_refinement       'Bruker XSCANS'
_computing_data_collection       'Bruker XSCANS'
_computing_data_reduction        'Bruker SHELXTL'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean none
_diffrn_measured_fraction_theta_full 0.982
_diffrn_measured_fraction_theta_max 0.982
_diffrn_measurement_device_type  'Bruker P4'
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0532
_diffrn_reflns_av_unetI/netI     0.0602
_diffrn_reflns_limit_h_max       22
_diffrn_reflns_limit_h_min       -19
_diffrn_reflns_limit_k_max       26
_diffrn_reflns_limit_k_min       -26
_diffrn_reflns_limit_l_max       22
_diffrn_reflns_limit_l_min       -22
_diffrn_reflns_number            43765
_diffrn_reflns_theta_full        27.50
_diffrn_reflns_theta_max         27.50
_diffrn_reflns_theta_min         2.01
_diffrn_source                   'fine-focus sealed tube'
_diffrn_standards_decay_%        none
_diffrn_standards_interval_count none
_diffrn_standards_interval_time  none
_diffrn_standards_number         none
_exptl_absorpt_coefficient_mu    9.909
_exptl_absorpt_correction_T_max  0.4087
_exptl_absorpt_correction_T_min  0.1826
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            COLOURLESS
_exptl_crystal_density_diffrn    2.757
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       BLOCK
_exptl_crystal_F_000             4400
_exptl_crystal_size_max          0.26
_exptl_crystal_size_mid          0.17
_exptl_crystal_size_min          0.11
_refine_diff_density_max         2.346
_refine_diff_density_min         -2.200
_refine_diff_density_rms         0.306
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.078
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     739
_refine_ls_number_reflns         12759
_refine_ls_number_restraints     2442
_refine_ls_restrained_S_all      1.014
_refine_ls_R_factor_all          0.0728
_refine_ls_R_factor_gt           0.0547
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0750P)²+26.2811P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1355
_refine_ls_wR_factor_ref         0.1504
_reflns_number_gt                10228
_reflns_number_total             12759
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic6b00754_si_010.cif
_cod_data_source_block           9
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_exptl_absorpt_correction_type' value 'MULTI-SCAN' was
changed to 'multi-scan' in accordance with the
/home/saulius/struct/COD-crude-data/automatic-downloads/DataCite-retrospective/ACS/depositions/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 last updated on
2011-04-26.

Automatic conversion script
Id: cif_fix_values 6909 2019-04-08 15:41:33Z antanas 
;
_cod_original_sg_symbol_H-M      P2(1)/c
_cod_database_code               4347890
_olex2_refinement_description
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H) groups, All C(H,H) groups, All O(H,H) groups
2. Uiso/Uaniso restraints and constraints
All non-hydrogen atoms have similar U: within 3.8A with sigma of 0.02 and sigma
for terminal atoms of 0.04
3. Others
 Fixed Sof: Tb2(0.9) Tb2'(0.1)
4.a Riding coordinates:
 O1W(H1A,H1B), O2W(H2A,H2B), O3W(H3A,H3B), O4W(H4A,H4B), O5W(H5A,H5B)
4.b Secondary CH2 refined with riding coordinates:
 C1(H1C,H1D), C2(H2C,H2D), C4(H4C,H4D), C5(H5D,H5C), C7(H7A,H7B), C8(H8A,H8B),
 C10(H10A,H10B), C11(H11A,H11B), C13(H13A,H13B), C14(H14A,H14B), C16(H16A,H16B),
  C17(H17A,H17B), C19(H19A,H19B), C20(H20A,H20B)
4.c Aromatic/amide H refined with riding coordinates:
 C24(H24), C25(H25), C26(H26), C27(H27)
;
_olex2_submission_special_instructions 'No special instructions were received'
loop_
_space_group_symop_id
_space_group_symop_operation_xyz
1 'x, y, z'
2 '-x, y+1/2, -z+1/2'
3 '-x, -y, -z'
4 'x, -y-1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
Ge1 Ge 0.49707(6) 0.71853(4) 0.98554(6) 0.0261(2) Uani 1 d . U
Ge2 Ge 0.62941(6) 0.66531(5) 1.16818(6) 0.0260(2) Uani 1 d . U
Ge3 Ge 0.58144(6) 0.55573(4) 1.27231(5) 0.0250(2) Uani 1 d . U
Ge4 Ge 0.39356(6) 0.49379(5) 1.18791(6) 0.0253(2) Uani 1 d . U
Ge5 Ge 0.25971(6) 0.54691(5) 1.00613(6) 0.0265(2) Uani 1 d . U
Ge6 Ge 0.30528(6) 0.65906(5) 0.90189(6) 0.0268(2) Uani 1 d . U
Ge7 Ge 0.21585(8) 0.60264(6) 0.61896(7) 0.0398(3) Uani 1 d . U
Tb1 Tb 0.41903(3) 0.65208(2) 1.12087(3) 0.03289(12) Uani 1 d . U
Tb2 Tb 0.06368(4) 0.49629(3) 0.64092(4) 0.02965(15) Uani 0.90 d . U
Tb3 Tb 0.28663(3) 0.50272(2) 0.81464(2) 0.02375(11) Uani 1 d . U
Tb4 Tb 0.33159(3) 0.38983(2) 0.99830(2) 0.02534(11) Uani 1 d . U
Tb5 Tb 0.54731(3) 0.38551(2) 1.18817(2) 0.02464(11) Uani 1 d . U
Tb2' Tb 0.0757(5) 0.5244(4) 0.6308(4) 0.0414(14) Uani 0.10 d . U
N1 N -0.0107(6) 0.4440(5) 0.7323(6) 0.0445(19) Uani 1 d . U
O1 O 0.5352(4) 0.7072(3) 1.0983(4) 0.0333(14) Uani 1 d . U
O2 O 0.5694(4) 0.6345(3) 1.2230(4) 0.0292(13) Uani 1 d . U
O3 O 0.4705(4) 0.5543(4) 1.2416(4) 0.0401(15) Uani 1 d . U
O4 O 0.3287(4) 0.5569(3) 1.1169(4) 0.0317(13) Uani 1 d . U
O5 O 0.2914(4) 0.6293(3) 0.9914(4) 0.0308(13) Uani 1 d . U
O6 O 0.3930(4) 0.7080(3) 0.9721(4) 0.0354(14) Uani 1 d . U
O7 O 0.5336(4) 0.6533(3) 0.9471(4) 0.0308(13) Uani 1 d . U
O8 O 0.6446(4) 0.5947(3) 1.1203(4) 0.0278(12) Uani 1 d . U
O9 O 0.5993(4) 0.4916(3) 1.2164(4) 0.0281(13) Uani 1 d . U
O10 O 0.4203(4) 0.4416(3) 1.1259(4) 0.0303(13) Uani 1 d . U
O11 O 0.3030(4) 0.4986(3) 0.9542(4) 0.0272(12) Uani 1 d . U
O12 O 0.3495(4) 0.6041(3) 0.8571(4) 0.0281(12) Uani 1 d . U
O13 O 0.4100(5) 0.7261(3) 0.8114(5) 0.0456(17) Uani 1 d . U
O14 O 0.3908(6) 0.8125(4) 0.7281(5) 0.059(2) Uani 1 d . U
O15 O 0.6803(4) 0.7133(3) 1.0744(4) 0.0352(14) Uani 1 d . U
O16 O 0.7695(6) 0.7897(4) 1.0794(5) 0.066(3) Uani 1 d . U
O17 O 0.7308(4) 0.5745(3) 1.2989(4) 0.0342(14) Uani 1 d . U
O18 O 0.8512(4) 0.5655(4) 1.4159(4) 0.0376(16) Uani 1 d . U
O19 O 0.5423(8) 0.3922(8) 1.4290(7) 0.117(4) Uani 1 d . U
O20 O 0.5132(6) 0.4221(5) 1.3005(5) 0.0585(19) Uani 1 d . U
O21 O 0.2461(4) 0.4402(3) 1.0559(4) 0.0351(14) Uani 1 d . U
O22 O 0.1478(5) 0.3815(5) 1.0717(6) 0.059(2) Uani 1 d . U
O23 O 0.1887(4) 0.5836(3) 0.8321(4) 0.0365(14) Uani 1 d . U
O24 O 0.0624(5) 0.5921(4) 0.7215(4) 0.0442(16) Uani 1 d . U
O25 O 0.0432(6) 0.5645(5) 0.5212(5) 0.0587(19) Uani 1 d . U
O26 O -0.0096(5) 0.6155(4) 0.4002(5) 0.054(2) Uani 1 d . U
O27 O 0.1823(4) 0.3846(4) 0.8864(4) 0.0388(15) Uani 1 d . U
O28 O 0.1518(4) 0.4473(3) 0.7720(4) 0.0367(15) Uani 1 d . U
O29 O 0.2153(6) 0.5635(5) 0.5273(5) 0.057(2) Uani 1 d . U
O30 O 0.1953(4) 0.5491(3) 0.6826(4) 0.0351(14) Uani 1 d . U
O31 O 0.3257(5) 0.6256(4) 0.6703(4) 0.0445(18) Uani 1 d . U
O1W O 0.4654(4) 0.5667(3) 1.0557(4) 0.0331(14) Uani 1 d . U
H1A H 0.4340 0.5378 1.0215 0.040 Uiso 1 d R .
H1B H 0.5152 0.5609 1.0612 0.040 Uiso 1 d R .
O2W O 0.3682(8) 0.7619(5) 1.1000(7) 0.094(3) Uani 1 d . U
H2A H 0.4010 0.7900 1.1346 0.112 Uiso 1 d R .
H2B H 0.3407 0.7813 1.0530 0.112 Uiso 1 d R .
O3W O 0.4465(7) 0.3039(5) 1.2147(7) 0.079(3) Uani 1 d . U
H3A H 0.4472 0.2810 1.2555 0.095 Uiso 1 d R .
H3B H 0.3977 0.3015 1.1737 0.095 Uiso 1 d R .
O4W O 0.2774(5) 0.3022(4) 1.0610(5) 0.0493(19) Uani 1 d . U
H4A H 0.2842 0.2632 1.0802 0.059 Uiso 1 d R .
H4B H 0.2400 0.3206 1.0720 0.059 Uiso 1 d R .
O5W O -0.0778(5) 0.5352(4) 0.5813(5) 0.0464(17) Uani 1 d . U
H5A H -0.1019 0.5461 0.5294 0.056 Uiso 1 d R .
H5B H -0.1012 0.5560 0.6074 0.056 Uiso 1 d R .
O6W O 0.0484(9) 0.3654(8) 0.1573(10) 0.128(6) Uani 1 d . U
O7W O 0.7016(12) 0.3714(17) 0.5454(13) 0.294(19) Uani 1 d . U
O8W O 0.9421(11) 0.7329(8) 0.2966(12) 0.148(6) Uani 1 d . U
O9W O 0.8548(10) 0.9036(7) 0.1689(8) 0.116(5) Uani 1 d . U
O10W O 0.9457(14) 0.7893(10) 0.1290(14) 0.201(7) Uani 1 d . U
C1 C 0.5169(7) 0.8050(4) 0.9532(6) 0.036(2) Uani 1 d . U
H1C H 0.5298 0.8349 1.0003 0.044 Uiso 1 calc R .
H1D H 0.5656 0.8033 0.9414 0.044 Uiso 1 calc R .
C2 C 0.4415(8) 0.8321(5) 0.8752(6) 0.041(2) Uani 1 d . U
H2C H 0.3947 0.8388 0.8893 0.049 Uiso 1 calc R .
H2D H 0.4565 0.8745 0.8603 0.049 Uiso 1 calc R .
C3 C 0.4140(7) 0.7866(5) 0.7998(6) 0.037(2) Uani 1 d . U
C4 C 0.7183(7) 0.7212(5) 1.2420(6) 0.037(2) Uani 1 d . U
H4C H 0.7052 0.7366 1.2872 0.045 Uiso 1 calc R .
H4D H 0.7701 0.6959 1.2675 0.045 Uiso 1 calc R .
C5 C 0.7317(8) 0.7804(6) 1.1958(6) 0.045(2) Uani 1 d . U
H5D H 0.6878 0.8127 1.1856 0.054 Uiso 1 calc R .
H5C H 0.7855 0.8008 1.2310 0.054 Uiso 1 calc R .
C6 C 0.7301(7) 0.7597(5) 1.1121(7) 0.040(2) Uani 1 d . U
C7 C 0.6403(6) 0.5594(5) 1.3943(6) 0.0360(19) Uani 1 d . U
H7A H 0.6045 0.5810 1.4157 0.043 Uiso 1 calc R .
H7B H 0.6501 0.5148 1.4163 0.043 Uiso 1 calc R .
C8 C 0.7253(7) 0.5960(6) 1.4280(6) 0.046(2) Uani 1 d . U
H8A H 0.7153 0.6431 1.4241 0.055 Uiso 1 calc R .
H8B H 0.7585 0.5849 1.4872 0.055 Uiso 1 calc R .
C9 C 0.7735(6) 0.5778(5) 1.3786(6) 0.0334(19) Uani 1 d . U
C10 C 0.3479(7) 0.4590(6) 1.2616(7) 0.045(2) Uani 1 d . U
H10A H 0.3040 0.4883 1.2603 0.054 Uiso 1 calc R .
H10B H 0.3222 0.4165 1.2399 0.054 Uiso 1 calc R .
C11 C 0.4135(8) 0.4506(7) 1.3531(7) 0.052(3) Uani 1 d . U
H11A H 0.3898 0.4240 1.3832 0.063 Uiso 1 calc R .
H11B H 0.4271 0.4934 1.3801 0.063 Uiso 1 calc R .
C12 C 0.4948(8) 0.4177(7) 1.3599(7) 0.053(2) Uani 1 d . U
C13 C 0.1421(7) 0.5441(6) 0.9821(7) 0.042(2) Uani 1 d . U
H13A H 0.1240 0.5879 0.9887 0.050 Uiso 1 calc R .
H13B H 0.1093 0.5309 0.9236 0.050 Uiso 1 calc R .
C14 C 0.1240(8) 0.4959(6) 1.0404(8) 0.049(2) Uani 1 d . U
H14A H 0.1365 0.5174 1.0939 0.059 Uiso 1 calc R .
H14B H 0.0647 0.4844 1.0143 0.059 Uiso 1 calc R .
C15 C 0.1767(7) 0.4330(6) 1.0568(7) 0.042(2) Uani 1 d . U
C16 C 0.2158(6) 0.7181(5) 0.8302(6) 0.039(2) Uani 1 d . U
H16A H 0.2198 0.7587 0.8608 0.047 Uiso 1 calc R .
H16B H 0.2239 0.7289 0.7804 0.047 Uiso 1 calc R .
C17 C 0.1273(7) 0.6891(5) 0.8018(7) 0.048(3) Uani 1 d . U
H17A H 0.1095 0.6956 0.8462 0.058 Uiso 1 calc R .
H17B H 0.0882 0.7123 0.7518 0.058 Uiso 1 calc R .
C18 C 0.1247(6) 0.6163(5) 0.7820(6) 0.0366(19) Uani 1 d . U
C19 C 0.1514(8) 0.6830(6) 0.5897(8) 0.054(3) Uani 1 d . U
H19A H 0.1457 0.6982 0.6393 0.065 Uiso 1 calc R .
H19B H 0.1833 0.7160 0.5763 0.065 Uiso 1 calc R .
C20 C 0.0670(11) 0.6792(8) 0.5188(11) 0.100(4) Uani 1 d . U
H20A H 0.0282 0.6976 0.5387 0.120 Uiso 1 calc R .
H20B H 0.0667 0.7087 0.4753 0.120 Uiso 1 calc R .
C21 C 0.0308(8) 0.6171(6) 0.4772(7) 0.049(2) Uani 1 d . U
C22 C 0.1312(6) 0.4120(5) 0.8218(6) 0.0350(18) Uani 1 d . U
C23 C 0.0411(7) 0.4084(6) 0.8008(6) 0.041(2) Uani 1 d . U
C24 C 0.0117(8) 0.3704(6) 0.8476(8) 0.054(3) Uani 1 d . U
H24 H 0.0499 0.3477 0.8948 0.065 Uiso 1 calc R .
C25 C -0.0730(8) 0.3656(7) 0.8255(9) 0.059(3) Uani 1 d . U
H25 H -0.0934 0.3398 0.8562 0.071 Uiso 1 calc R .
C26 C -0.1269(9) 0.4015(7) 0.7542(9) 0.065(3) Uani 1 d . U
H26 H -0.1848 0.4002 0.7364 0.078 Uiso 1 calc R .
C27 C -0.0929(8) 0.4393(6) 0.7102(8) 0.054(3) Uani 1 d . U
H27 H -0.1297 0.4625 0.6628 0.065 Uiso 1 calc R .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ge Ge 0.1547 1.8001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Tb Tb -0.1723 4.1537 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O1 Ge1 C1 114.3(4) . .
O6 Ge1 O1 89.9(3) . .
O6 Ge1 C1 112.7(4) . .
O7 Ge1 O1 107.8(3) . .
O7 Ge1 O6 113.5(3) . .
O7 Ge1 C1 115.8(4) . .
Tb1 Ge2 Tb4 111.23(3) . 3_667
O1 Ge2 Tb1 44.9(2) . .
O1 Ge2 Tb4 92.5(2) . 3_667
O1 Ge2 O2 86.8(3) . .
O1 Ge2 C4 115.1(4) . .
O2 Ge2 Tb1 44.51(19) . .
O2 Ge2 Tb4 135.1(2) . 3_667
O2 Ge2 C4 109.9(4) . .
O8 Ge2 Tb1 101.4(2) . .
O8 Ge2 Tb4 36.69(19) . 3_667
O8 Ge2 O1 110.7(3) . .
O8 Ge2 O2 102.7(3) . .
O8 Ge2 C4 124.2(4) . .
C4 Ge2 Tb1 133.6(3) . .
C4 Ge2 Tb4 110.9(3) . 3_667
O2 Ge3 O3 89.1(3) . .
O2 Ge3 C7 113.3(4) . .
O3 Ge3 C7 108.8(4) . .
O9 Ge3 O2 114.1(3) . .
O9 Ge3 O3 105.2(3) . .
O9 Ge3 C7 120.8(4) . .
O3 Ge4 O4 89.0(3) . .
O3 Ge4 C10 110.2(4) . .
O4 Ge4 C10 113.4(4) . .
O10 Ge4 O3 113.8(3) . .
O10 Ge4 O4 105.4(3) . .
O10 Ge4 C10 120.5(4) . .
Tb1 Ge5 Tb4 112.32(3) . .
O4 Ge5 Tb1 45.2(2) . .
O4 Ge5 Tb4 93.5(2) . .
O4 Ge5 O5 86.8(3) . .
O4 Ge5 C13 113.2(4) . .
O5 Ge5 Tb1 44.00(19) . .
O5 Ge5 Tb4 134.6(2) . .
O5 Ge5 C13 111.4(4) . .
O11 Ge5 Tb1 103.1(2) . .
O11 Ge5 Tb4 37.0(2) . .
O11 Ge5 O4 112.9(3) . .
O11 Ge5 O5 102.3(3) . .
O11 Ge5 C13 123.3(4) . .
C13 Ge5 Tb1 132.8(4) . .
C13 Ge5 Tb4 110.0(3) . .
Tb1 Ge6 Tb3 110.35(3) . .
O5 Ge6 Tb1 41.7(2) . .
O5 Ge6 Tb3 93.2(2) . .
O5 Ge6 C16 113.0(4) . .
O6 Ge6 Tb1 49.9(2) . .
O6 Ge6 Tb3 133.9(2) . .
O6 Ge6 O5 89.5(3) . .
O6 Ge6 C16 108.4(4) . .
O12 Ge6 Tb1 108.6(2) . .
O12 Ge6 Tb3 35.7(2) . .
O12 Ge6 O5 116.1(3) . .
O12 Ge6 O6 104.1(3) . .
O12 Ge6 C16 120.1(4) . .
C16 Ge6 Tb1 130.9(3) . .
C16 Ge6 Tb3 112.6(3) . .
O29 Ge7 Tb2' 98.4(3) . .
O29 Ge7 O31 98.4(4) . .
O29 Ge7 C19 111.4(5) . .
O30 Ge7 Tb2' 37.5(3) . .
O30 Ge7 O29 112.7(4) . .
O30 Ge7 O31 109.0(3) . .
O30 Ge7 C19 116.4(5) . .
O31 Ge7 Tb2' 146.5(3) . .
O31 Ge7 C19 107.1(5) . .
C19 Ge7 Tb2' 93.3(4) . .
Ge2 Tb1 Ge6 107.70(3) . .
Ge5 Tb1 Ge2 135.81(3) . .
Ge5 Tb1 Ge6 56.11(2) . .
O1 Tb1 Ge2 30.19(14) . .
O1 Tb1 Ge5 134.93(15) . .
O1 Tb1 Ge6 85.66(14) . .
O1 Tb1 O3 115.1(2) . .
O1 Tb1 O6 57.7(2) . .
O2 Tb1 Ge2 30.86(14) . .
O2 Tb1 Ge5 132.84(15) . .
O2 Tb1 Ge6 135.99(14) . .
O2 Tb1 O1 59.5(2) . .
O2 Tb1 O3 56.9(2) . .
O2 Tb1 O6 115.7(2) . .
O3 Tb1 Ge2 84.96(15) . .
O3 Tb1 Ge5 84.99(15) . .
O3 Tb1 Ge6 135.88(14) . .
O4 Tb1 Ge2 132.72(15) . .
O4 Tb1 Ge5 30.87(14) . .
O4 Tb1 Ge6 86.98(14) . .
O4 Tb1 O1 154.0(2) . .
O4 Tb1 O2 112.1(2) . .
O4 Tb1 O3 56.9(2) . .
O4 Tb1 O6 117.7(2) . .
O5 Tb1 Ge2 134.20(15) . .
O5 Tb1 Ge5 31.09(15) . .
O5 Tb1 Ge6 29.26(15) . .
O5 Tb1 O1 114.9(2) . .
O5 Tb1 O2 154.1(2) . .
O5 Tb1 O3 116.1(2) . .
O5 Tb1 O4 60.5(2) . .
O5 Tb1 O6 58.8(2) . .
O6 Tb1 Ge2 84.83(15) . .
O6 Tb1 Ge5 86.79(15) . .
O6 Tb1 Ge6 30.70(15) . .
O6 Tb1 O3 155.31(19) . .
O14 Tb1 Ge2 112.4(3) 4_576 .
O14 Tb1 Ge5 105.5(3) 4_576 .
O14 Tb1 Ge6 132.5(2) 4_576 .
O14 Tb1 O1 118.7(3) 4_576 .
O14 Tb1 O2 90.0(3) 4_576 .
O14 Tb1 O3 73.0(2) 4_576 .
O14 Tb1 O4 84.2(3) 4_576 .
O14 Tb1 O5 112.6(3) 4_576 .
O14 Tb1 O6 131.7(2) 4_576 .
O14 Tb1 O1W 150.2(3) 4_576 .
O14 Tb1 O2W 67.9(3) 4_576 .
O1W Tb1 Ge2 67.41(17) . .
O1W Tb1 Ge5 68.40(17) . .
O1W Tb1 Ge6 69.86(15) . .
O1W Tb1 O1 77.0(2) . .
O1W Tb1 O2 76.3(2) . .
O1W Tb1 O3 77.3(2) . .
O1W Tb1 O4 77.0(2) . .
O1W Tb1 O5 77.8(2) . .
O1W Tb1 O6 78.0(2) . .
O2W Tb1 Ge2 105.0(3) . .
O2W Tb1 Ge5 109.8(3) . .
O2W Tb1 Ge6 78.1(3) . .
O2W Tb1 O1 80.6(3) . .
O2W Tb1 O2 117.2(4) . .
O2W Tb1 O3 140.6(3) . .
O2W Tb1 O4 122.1(4) . .
O2W Tb1 O5 84.3(4) . .
O2W Tb1 O6 64.0(3) . .
O2W Tb1 O1W 141.9(3) . .
Tb2' Tb2 Tb3 81.0(6) . .
Tb2' Tb2 N1 143.0(7) . .
Tb2' Tb2 O18 90.3(7) . 3_667
Tb2' Tb2 O24 63.1(7) . .
Tb2' Tb2 O25 37.9(6) . .
Tb2' Tb2 O25 104.5(6) . 3_566
Tb2' Tb2 O26 148.6(7) . 3_566
Tb2' Tb2 O28 118.3(6) . .
Tb2' Tb2 O30 45.8(6) . .
Tb2' Tb2 O5W 89.7(7) . .
N1 Tb2 Tb3 98.02(19) . .
N1 Tb2 O25 98.0(3) . 3_566
O18 Tb2 Tb3 75.05(15) 3_667 .
O18 Tb2 N1 125.4(3) 3_667 .
O18 Tb2 O25 68.9(2) 3_667 3_566
O24 Tb2 Tb3 76.84(17) . .
O24 Tb2 N1 80.6(3) . .
O24 Tb2 O18 143.9(2) . 3_667
O24 Tb2 O25 90.7(3) . .
O24 Tb2 O25 138.3(2) . 3_566
O24 Tb2 O26 145.0(3) . 3_566
O25 Tb2 Tb3 113.0(2) . .
O25 Tb2 Tb3 143.45(17) 3_566 .
O25 Tb2 N1 145.0(3) . .
O25 Tb2 O18 80.0(3) . 3_667
O25 Tb2 O25 66.7(3) . 3_566
O25 Tb2 O26 112.7(3) . 3_566
O26 Tb2 Tb3 113.86(18) 3_566 .
O26 Tb2 N1 65.3(3) 3_566 .
O26 Tb2 O18 68.8(3) 3_566 3_667
O26 Tb2 O25 46.8(2) 3_566 3_566
O28 Tb2 Tb3 38.62(17) . .
O28 Tb2 N1 62.5(3) . .
O28 Tb2 O18 85.6(2) . 3_667
O28 Tb2 O24 86.5(2) . .
O28 Tb2 O25 151.2(3) . .
O28 Tb2 O25 130.0(2) . 3_566
O28 Tb2 O26 84.5(2) . 3_566
O28 Tb2 O30 75.5(2) . .
O28 Tb2 O5W 133.3(3) . .
O30 Tb2 Tb3 36.90(15) . .
O30 Tb2 N1 131.5(2) . .
O30 Tb2 O18 70.6(2) . 3_667
O30 Tb2 O24 73.3(2) . .
O30 Tb2 O25 128.5(2) . 3_566
O30 Tb2 O25 76.2(3) . .
O30 Tb2 O26 135.7(3) . 3_566
O30 Tb2 O5W 133.2(3) . .
O5W Tb2 Tb3 149.78(18) . .
O5W Tb2 N1 72.7(3) . .
O5W Tb2 O18 134.0(2) . 3_667
O5W Tb2 O24 73.3(2) . .
O5W Tb2 O25 66.7(2) . 3_566
O5W Tb2 O25 72.4(3) . .
O5W Tb2 O26 88.8(3) . 3_566
Ge6 Tb3 Tb4 103.62(3) . .
Ge6 Tb3 Tb5 61.72(2) . 3_667
Ge6 Tb3 Tb2' 98.04(11) . .
Tb5 Tb3 Tb4 120.811(17) 3_667 .
Tb5 Tb3 Tb2' 114.18(13) 3_667 .
Tb2' Tb3 Tb4 124.85(13) . .
O8 Tb3 Ge6 128.87(15) 3_667 .
O8 Tb3 Tb4 36.27(15) 3_667 .
O8 Tb3 Tb5 106.14(16) 3_667 3_667
O8 Tb3 Tb2' 128.99(19) 3_667 .
O8 Tb3 O17 73.1(2) 3_667 3_667
O8 Tb3 O23 137.3(2) 3_667 .
O8 Tb3 O28 89.3(2) 3_667 .
O8 Tb3 O30 143.2(2) 3_667 .
O9 Tb3 Ge6 97.71(15) 3_667 .
O9 Tb3 Tb4 110.82(15) 3_667 .
O9 Tb3 Tb5 36.22(15) 3_667 3_667
O9 Tb3 Tb2' 115.65(19) 3_667 .
O9 Tb3 O8 80.6(2) 3_667 3_667
O9 Tb3 O11 121.9(2) 3_667 .
O9 Tb3 O17 69.6(2) 3_667 3_667
O9 Tb3 O23 135.9(2) 3_667 .
O9 Tb3 O28 141.9(2) 3_667 .
O9 Tb3 O30 92.3(2) 3_667 .
O11 Tb3 Ge6 68.07(15) . .
O11 Tb3 Tb4 36.33(14) . .
O11 Tb3 Tb5 107.34(16) . 3_667
O11 Tb3 Tb2' 121.9(2) . .
O11 Tb3 O8 70.1(2) . 3_667
O11 Tb3 O17 138.1(2) . 3_667
O11 Tb3 O23 70.8(2) . .
O11 Tb3 O28 87.8(2) . .
O11 Tb3 O30 139.5(2) . .
O12 Tb3 Ge6 26.09(16) . .
O12 Tb3 Tb4 112.18(15) . .
O12 Tb3 Tb5 35.77(16) . 3_667
O12 Tb3 Tb2' 109.37(19) . .
O12 Tb3 O8 121.6(2) . 3_667
O12 Tb3 O9 71.6(2) . 3_667
O12 Tb3 O11 82.6(2) . .
O12 Tb3 O17 135.0(2) . 3_667
O12 Tb3 O23 68.5(2) . .
O12 Tb3 O28 141.3(2) . .
O12 Tb3 O30 89.2(2) . .
O17 Tb3 Ge6 153.85(16) 3_667 .
O17 Tb3 Tb4 102.30(16) 3_667 .
O17 Tb3 Tb5 101.47(17) 3_667 3_667
O17 Tb3 Tb2' 69.45(19) 3_667 .
O17 Tb3 O23 132.3(2) 3_667 .
O23 Tb3 Ge6 44.21(17) . .
O23 Tb3 Tb4 101.20(16) . .
O23 Tb3 Tb5 101.06(17) . 3_667
O23 Tb3 Tb2' 63.07(19) . .
O28 Tb3 Ge6 116.65(17) . .
O28 Tb3 Tb4 78.04(16) . .
O28 Tb3 Tb5 161.15(16) . 3_667
O28 Tb3 Tb2' 47.0(2) . .
O28 Tb3 O17 72.3(2) . 3_667
O28 Tb3 O23 72.9(2) . .
O30 Tb3 Ge6 87.76(17) . .
O30 Tb3 Tb4 152.18(18) . .
O30 Tb3 Tb5 86.97(18) . 3_667
O30 Tb3 Tb2' 27.4(2) . .
O30 Tb3 O17 70.6(2) . 3_667
O30 Tb3 O23 69.3(2) . .
O30 Tb3 O28 74.2(2) . .
Ge2 Tb4 Tb3 61.15(3) 3_667 .
Ge2 Tb4 Tb5 103.84(3) 3_667 .
Ge5 Tb4 Ge2 122.87(3) . 3_667
Ge5 Tb4 Tb3 61.76(2) . .
Ge5 Tb4 Tb5 103.31(2) . .
Tb3 Tb4 Tb5 121.436(19) . .
O7 Tb4 Ge2 71.32(15) 3_667 3_667
O7 Tb4 Ge5 131.43(16) 3_667 .
O7 Tb4 Tb3 112.36(16) 3_667 .
O7 Tb4 Tb5 34.48(15) 3_667 .
O7 Tb4 O8 82.3(2) 3_667 3_667
O7 Tb4 O10 68.8(2) 3_667 .
O7 Tb4 O11 122.2(2) 3_667 .
O7 Tb4 O15 74.1(2) 3_667 3_667
O7 Tb4 O21 135.6(2) 3_667 .
O7 Tb4 O27 147.9(2) 3_667 .
O7 Tb4 O4W 94.1(3) 3_667 .
O8 Tb4 Ge2 26.63(15) 3_667 3_667
O8 Tb4 Ge5 97.17(15) 3_667 .
O8 Tb4 Tb3 36.66(15) 3_667 .
O8 Tb4 Tb5 106.54(16) 3_667 .
O8 Tb4 O10 119.3(2) 3_667 .
O8 Tb4 O11 70.7(2) 3_667 .
O8 Tb4 O15 69.5(2) 3_667 3_667
O8 Tb4 O21 136.1(2) 3_667 .
O8 Tb4 O27 81.0(2) 3_667 .
O8 Tb4 O4W 138.5(2) 3_667 .
O10 Tb4 Ge2 130.80(16) . 3_667
O10 Tb4 Ge5 69.64(16) . .
O10 Tb4 Tb3 110.44(16) . .
O10 Tb4 Tb5 35.00(16) . .
O10 Tb4 O15 139.6(2) . 3_667
O10 Tb4 O21 71.6(2) . .
O10 Tb4 O27 143.2(2) . .
O10 Tb4 O4W 97.1(2) . .
O11 Tb4 Ge2 96.90(15) . 3_667
O11 Tb4 Ge5 26.59(15) . .
O11 Tb4 Tb3 36.66(14) . .
O11 Tb4 Tb5 107.59(16) . .
O11 Tb4 O10 81.3(2) . .
O11 Tb4 O15 133.8(2) . 3_667
O11 Tb4 O21 69.4(2) . .
O11 Tb4 O27 77.2(2) . .
O11 Tb4 O4W 139.2(3) . .
O15 Tb4 Ge2 43.72(16) 3_667 3_667
O15 Tb4 Ge5 150.78(16) 3_667 .
O15 Tb4 Tb3 97.95(16) 3_667 .
O15 Tb4 Tb5 105.40(16) 3_667 .
O15 Tb4 O27 74.3(2) 3_667 .
O15 Tb4 O4W 69.7(2) 3_667 .
O21 Tb4 Ge2 153.11(17) . 3_667
O21 Tb4 Ge5 43.61(16) . .
O21 Tb4 Tb3 99.65(17) . .
O21 Tb4 Tb5 102.39(17) . .
O21 Tb4 O15 132.2(2) . 3_667
O21 Tb4 O27 73.0(2) . .
O21 Tb4 O4W 71.5(3) . .
O27 Tb4 Ge2 81.60(17) . 3_667
O27 Tb4 Ge5 77.98(17) . .
O27 Tb4 Tb3 66.23(16) . .
O27 Tb4 Tb5 172.02(16) . .
O4W Tb4 Ge2 113.45(19) . 3_667
O4W Tb4 Ge5 114.97(19) . .
O4W Tb4 Tb3 147.00(19) . .
O4W Tb4 Tb5 91.55(19) . .
O4W Tb4 O27 80.9(3) . .
Tb3 Tb5 Tb4 117.75(2) 3_667 .
O7 Tb5 Tb3 109.31(17) 3_667 3_667
O7 Tb5 Tb4 34.54(16) 3_667 .
O7 Tb5 O10 69.3(2) 3_667 .
O7 Tb5 O13 74.4(2) 3_667 3_667
O7 Tb5 O20 132.9(3) 3_667 .
O7 Tb5 O31 149.8(2) 3_667 3_667
O7 Tb5 O3W 78.7(3) 3_667 .
O9 Tb5 Tb3 36.20(16) . 3_667
O9 Tb5 Tb4 108.53(16) . .
O9 Tb5 O7 123.2(2) . 3_667
O9 Tb5 O10 81.6(2) . .
O9 Tb5 O13 142.1(3) . 3_667
O9 Tb5 O20 75.9(3) . .
O9 Tb5 O31 76.9(2) . 3_667
O9 Tb5 O3W 142.1(3) . .
O10 Tb5 Tb3 107.38(17) . 3_667
O10 Tb5 Tb4 35.49(15) . .
O10 Tb5 O13 135.0(2) . 3_667
O10 Tb5 O20 72.5(3) . .
O10 Tb5 O31 140.1(2) . 3_667
O10 Tb5 O3W 78.6(3) . .
O12 Tb5 Tb3 35.93(15) 3_667 3_667
O12 Tb5 Tb4 109.64(15) 3_667 .
O12 Tb5 O7 84.4(2) 3_667 3_667
O12 Tb5 O9 71.8(2) 3_667 .
O12 Tb5 O10 122.8(2) 3_667 .
O12 Tb5 O13 77.9(2) 3_667 3_667
O12 Tb5 O20 140.7(3) 3_667 .
O12 Tb5 O31 81.4(2) 3_667 3_667
O12 Tb5 O3W 145.6(3) 3_667 .
O13 Tb5 Tb3 109.2(2) 3_667 3_667
O13 Tb5 Tb4 102.60(18) 3_667 .
O13 Tb5 O20 118.7(3) 3_667 .
O13 Tb5 O31 76.6(3) 3_667 3_667
O13 Tb5 O3W 68.7(3) 3_667 .
O20 Tb5 Tb3 107.6(2) . 3_667
O20 Tb5 Tb4 101.3(2) . .
O20 Tb5 O31 69.8(3) . 3_667
O20 Tb5 O3W 67.5(3) . .
O31 Tb5 Tb3 72.68(17) 3_667 3_667
O31 Tb5 Tb4 168.62(17) 3_667 .
O31 Tb5 O3W 98.5(3) 3_667 .
O3W Tb5 Tb3 171.2(2) . 3_667
O3W Tb5 Tb4 70.9(2) . .
Ge7 Tb2' Tb3 65.48(14) . .
Tb2 Tb2' Ge7 147.4(8) . .
Tb2 Tb2' Tb3 89.0(6) . .
Tb2 Tb2' O18 74.8(7) . 3_667
Tb2 Tb2' O24 101.4(8) . .
Tb2 Tb2' O25 130.0(8) . .
Tb2 Tb2' O28 49.5(5) . .
Tb2 Tb2' O30 120.3(8) . .
Tb2 Tb2' O5W 74.8(7) . .
O18 Tb2' Ge7 79.1(3) 3_667 .
O18 Tb2' Tb3 75.1(2) 3_667 .
O18 Tb2' O28 76.5(3) 3_667 .
O24 Tb2' Ge7 94.1(3) . .
O24 Tb2' Tb3 80.2(3) . .
O24 Tb2' O18 155.0(4) . 3_667
O24 Tb2' O28 82.3(3) . .
O24 Tb2' O5W 75.5(3) . .
O25 Tb2' Ge7 66.8(4) . .
O25 Tb2' Tb3 131.3(4) . .
O25 Tb2' O18 87.3(4) . 3_667
O25 Tb2' O24 112.3(5) . .
O25 Tb2' O28 163.4(5) . .
O25 Tb2' O30 98.3(5) . .
O25 Tb2' O5W 79.0(4) . .
O28 Tb2' Ge7 105.7(3) . .
O28 Tb2' Tb3 40.62(17) . .
O30 Tb2' Ge7 31.9(2) . .
O30 Tb2' Tb3 33.6(2) . .
O30 Tb2' O18 75.0(3) . 3_667
O30 Tb2' O24 86.5(4) . .
O30 Tb2' O28 74.0(3) . .
O30 Tb2' O5W 158.9(5) . .
O5W Tb2' Ge7 137.3(4) . .
O5W Tb2' Tb3 147.2(3) . .
O5W Tb2' O18 125.4(4) . 3_667
O5W Tb2' O28 113.5(4) . .
C23 N1 Tb2 115.0(7) . .
C27 N1 Tb2 127.4(8) . .
C27 N1 C23 116.5(10) . .
Ge1 O1 Tb1 106.9(3) . .
Ge2 O1 Ge1 126.8(4) . .
Ge2 O1 Tb1 104.9(3) . .
Ge2 O2 Tb1 104.6(2) . .
Ge3 O2 Ge2 126.1(4) . .
Ge3 O2 Tb1 109.9(3) . .
Ge3 O3 Tb1 99.8(3) . .
Ge4 O3 Ge3 131.0(4) . .
Ge4 O3 Tb1 100.0(3) . .
Ge4 O4 Tb1 109.1(3) . .
Ge5 O4 Ge4 126.2(4) . .
Ge5 O4 Tb1 103.9(3) . .
Ge5 O5 Tb1 104.9(3) . .
Ge6 O5 Ge5 127.0(4) . .
Ge6 O5 Tb1 109.1(3) . .
Ge1 O6 Ge6 134.0(4) . .
Ge1 O6 Tb1 101.3(3) . .
Ge6 O6 Tb1 99.4(3) . .
Ge1 O7 Tb4 128.2(3) . 3_667
Ge1 O7 Tb5 119.5(3) . 3_667
Tb5 O7 Tb4 111.0(3) 3_667 3_667
Ge2 O8 Tb3 128.1(3) . 3_667
Ge2 O8 Tb4 116.7(3) . 3_667
Tb4 O8 Tb3 107.1(3) 3_667 3_667
Ge3 O9 Tb3 119.2(3) . 3_667
Ge3 O9 Tb5 131.8(3) . .
Tb3 O9 Tb5 107.6(2) 3_667 .
Ge4 O10 Tb4 128.6(3) . .
Ge4 O10 Tb5 118.6(3) . .
Tb5 O10 Tb4 109.5(3) . .
Ge5 O11 Tb3 130.7(3) . .
Ge5 O11 Tb4 116.4(3) . .
Tb4 O11 Tb3 107.0(2) . .
Ge6 O12 Tb3 118.2(3) . .
Ge6 O12 Tb5 132.9(3) . 3_667
Tb5 O12 Tb3 108.3(2) 3_667 .
C3 O13 Tb5 153.0(8) . 3_667
C3 O14 Tb1 150.8(9) . 4_575
C6 O15 Tb4 143.6(7) . 3_667
C9 O17 Tb3 137.3(6) . 3_667
Tb2 O18 Tb2' 14.89(18) 3_667 3_667
C9 O18 Tb2 127.3(6) . 3_667
C9 O18 Tb2' 124.1(6) . 3_667
C12 O20 Tb5 158.0(9) . .
C15 O21 Tb4 140.1(7) . .
C18 O23 Tb3 135.3(6) . .
Tb2' O24 Tb2 15.6(2) . .
C18 O24 Tb2 125.9(6) . .
C18 O24 Tb2' 122.0(7) . .
Tb2 O25 Tb2 113.3(3) . 3_566
Tb2' O25 Tb2 12.1(2) . .
Tb2' O25 Tb2 125.3(5) . 3_566
C21 O25 Tb2 84.0(7) . 3_566
C21 O25 Tb2 158.1(8) . .
C21 O25 Tb2' 148.4(9) . .
C21 O26 Tb2 108.4(8) . 3_566
C22 O27 Tb4 143.0(7) . .
Tb2 O28 Tb3 104.1(3) . .
Tb2 O28 Tb2' 12.25(16) . .
Tb3 O28 Tb2' 92.4(3) . .
C22 O28 Tb2 129.0(6) . .
C22 O28 Tb3 124.9(6) . .
C22 O28 Tb2' 138.9(6) . .
Ge7 O30 Tb2 123.2(3) . .
Ge7 O30 Tb3 130.3(4) . .
Ge7 O30 Tb2' 110.7(4) . .
Tb3 O30 Tb2 106.2(3) . .
Tb2' O30 Tb2 13.9(2) . .
Tb2' O30 Tb3 119.0(4) . .
Ge7 O31 Tb5 140.0(4) . 3_667
Tb1 O1W H1A 125.5 . .
Tb1 O1W H1B 126.6 . .
H1A O1W H1B 107.9 . .
Tb1 O2W H2A 115.3 . .
Tb1 O2W H2B 127.0 . .
H2A O2W H2B 107.8 . .
Tb5 O3W H3A 137.4 . .
Tb5 O3W H3B 113.7 . .
H3A O3W H3B 108.6 . .
Tb4 O4W H4A 145.7 . .
Tb4 O4W H4B 105.9 . .
H4A O4W H4B 107.9 . .
Tb2 O5W Tb2' 15.50(18) . .
Tb2 O5W H5A 119.6 . .
Tb2 O5W H5B 126.2 . .
Tb2' O5W H5A 111.0 . .
Tb2' O5W H5B 124.8 . .
H5A O5W H5B 108.5 . .
Ge1 C1 H1C 109.0 . .
Ge1 C1 H1D 109.0 . .
H1C C1 H1D 107.8 . .
C2 C1 Ge1 113.0(7) . .
C2 C1 H1C 109.0 . .
C2 C1 H1D 109.0 . .
C1 C2 H2C 109.1 . .
C1 C2 H2D 109.1 . .
H2C C2 H2D 107.8 . .
C3 C2 C1 112.6(9) . .
C3 C2 H2C 109.1 . .
C3 C2 H2D 109.1 . .
O13 C3 O14 123.9(10) . .
O13 C3 C2 118.4(9) . .
O14 C3 C2 117.5(9) . .
Ge2 C4 H4C 109.1 . .
Ge2 C4 H4D 109.1 . .
H4C C4 H4D 107.9 . .
C5 C4 Ge2 112.3(7) . .
C5 C4 H4C 109.1 . .
C5 C4 H4D 109.1 . .
C4 C5 H5D 109.5 . .
C4 C5 H5C 109.5 . .
H5D C5 H5C 108.1 . .
C6 C5 C4 110.8(9) . .
C6 C5 H5D 109.5 . .
C6 C5 H5C 109.5 . .
O15 C6 C5 115.4(10) . .
O16 C6 O15 121.9(10) . .
O16 C6 C5 122.4(10) . .
Ge3 C7 H7A 108.8 . .
Ge3 C7 H7B 108.8 . .
H7A C7 H7B 107.7 . .
C8 C7 Ge3 114.0(7) . .
C8 C7 H7A 108.8 . .
C8 C7 H7B 108.8 . .
C7 C8 H8A 109.4 . .
C7 C8 H8B 109.4 . .
H8A C8 H8B 108.0 . .
C9 C8 C7 111.2(8) . .
C9 C8 H8A 109.4 . .
C9 C8 H8B 109.4 . .
O17 C9 C8 115.9(9) . .
O18 C9 O17 123.3(9) . .
O18 C9 C8 120.8(8) . .
Ge4 C10 H10A 108.9 . .
Ge4 C10 H10B 108.9 . .
H10A C10 H10B 107.7 . .
C11 C10 Ge4 113.6(8) . .
C11 C10 H10A 108.9 . .
C11 C10 H10B 108.9 . .
C10 C11 H11A 109.1 . .
C10 C11 H11B 109.1 . .
C10 C11 C12 112.5(10) . .
H11A C11 H11B 107.8 . .
C12 C11 H11A 109.1 . .
C12 C11 H11B 109.1 . .
O19 C12 C11 117.5(12) . .
O20 C12 O19 123.0(13) . .
O20 C12 C11 119.2(10) . .
Ge5 C13 H13A 109.0 . .
Ge5 C13 H13B 109.0 . .
H13A C13 H13B 107.8 . .
C14 C13 Ge5 112.8(7) . .
C14 C13 H13A 109.0 . .
C14 C13 H13B 109.0 . .
C13 C14 H14A 109.3 . .
C13 C14 H14B 109.3 . .
H14A C14 H14B 108.0 . .
C15 C14 C13 111.5(9) . .
C15 C14 H14A 109.3 . .
C15 C14 H14B 109.3 . .
O21 C15 C14 115.0(10) . .
O22 C15 O21 126.9(11) . .
O22 C15 C14 118.0(10) . .
Ge6 C16 H16A 108.9 . .
Ge6 C16 H16B 108.9 . .
H16A C16 H16B 107.7 . .
C17 C16 Ge6 113.4(7) . .
C17 C16 H16A 108.9 . .
C17 C16 H16B 108.9 . .
C16 C17 H17A 109.2 . .
C16 C17 H17B 109.2 . .
H17A C17 H17B 107.9 . .
C18 C17 C16 112.0(9) . .
C18 C17 H17A 109.2 . .
C18 C17 H17B 109.2 . .
O23 C18 C17 114.9(9) . .
O24 C18 O23 124.6(10) . .
O24 C18 C17 120.5(9) . .
Ge7 C19 H19A 108.2 . .
Ge7 C19 H19B 108.2 . .
H19A C19 H19B 107.3 . .
C20 C19 Ge7 116.4(10) . .
C20 C19 H19A 108.2 . .
C20 C19 H19B 108.2 . .
C19 C20 H20A 106.8 . .
C19 C20 H20B 106.8 . .
H20A C20 H20B 106.7 . .
C21 C20 C19 122.1(13) . .
C21 C20 H20A 106.8 . .
C21 C20 H20B 106.8 . .
O25 C21 C20 119.8(12) . .
O26 C21 O25 120.6(11) . .
O26 C21 C20 119.6(12) . .
O27 C22 O28 124.2(10) . .
O27 C22 C23 119.0(9) . .
O28 C22 C23 116.8(9) . .
N1 C23 C22 115.6(10) . .
N1 C23 C24 122.7(11) . .
C24 C23 C22 121.7(10) . .
C23 C24 H24 119.4 . .
C25 C24 C23 121.1(12) . .
C25 C24 H24 119.4 . .
C24 C25 H25 121.8 . .
C24 C25 C26 116.5(13) . .
C26 C25 H25 121.8 . .
C25 C26 H26 120.3 . .
C25 C26 C27 119.4(13) . .
C27 C26 H26 120.3 . .
N1 C27 C26 123.7(12) . .
N1 C27 H27 118.1 . .
C26 C27 H27 118.1 . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Ge1 O1 1.807(6) .
Ge1 O6 1.761(7) .
Ge1 O7 1.734(6) .
Ge1 C1 1.924(9) .
Ge2 Tb1 3.4449(15) .
Ge2 Tb4 3.4700(13) 3_667
Ge2 O1 1.793(7) .
Ge2 O2 1.826(7) .
Ge2 O8 1.741(6) .
Ge2 C4 1.912(10) .
Ge3 O2 1.787(6) .
Ge3 O3 1.790(7) .
Ge3 O9 1.741(6) .
Ge3 C7 1.931(9) .
Ge4 O3 1.768(7) .
Ge4 O4 1.807(6) .
Ge4 O10 1.727(6) .
Ge4 C10 1.933(10) .
Ge5 Tb1 3.4032(12) .
Ge5 Tb4 3.4582(13) .
Ge5 O4 1.799(6) .
Ge5 O5 1.819(7) .
Ge5 O11 1.729(6) .
Ge5 C13 1.931(11) .
Ge6 Tb1 3.4777(14) .
Ge6 Tb3 3.4782(13) .
Ge6 O5 1.798(6) .
Ge6 O6 1.799(7) .
Ge6 O12 1.736(6) .
Ge6 C16 1.945(9) .
Ge7 Tb2' 3.024(8) .
Ge7 O29 1.792(8) .
Ge7 O30 1.707(7) .
Ge7 O31 1.807(7) .
Ge7 C19 1.927(12) .
Tb1 O1 2.515(7) .
Tb1 O2 2.496(6) .
Tb1 O3 2.753(8) .
Tb1 O4 2.487(7) .
Tb1 O5 2.446(6) .
Tb1 O6 2.698(7) .
Tb1 O14 2.266(8) 4_576
Tb1 O1W 2.410(6) .
Tb1 O2W 2.373(9) .
Tb2 Tb3 3.7848(11) .
Tb2 Tb2' 0.660(8) .
Tb2 N1 2.697(10) .
Tb2 O18 2.477(7) 3_667
Tb2 O24 2.412(7) .
Tb2 O25 2.410(8) .
Tb2 O25 2.915(9) 3_566
Tb2 O26 2.446(8) 3_566
Tb2 O28 2.363(7) .
Tb2 O30 2.368(7) .
Tb2 O5W 2.383(7) .
Tb3 Tb4 3.7489(10) .
Tb3 Tb5 3.7259(10) 3_667
Tb3 Tb2' 3.739(7) .
Tb3 O8 2.342(6) 3_667
Tb3 O9 2.308(6) 3_667
Tb3 O11 2.341(6) .
Tb3 O12 2.303(6) .
Tb3 O17 2.449(6) 3_667
Tb3 O23 2.500(7) .
Tb3 O28 2.436(7) .
Tb3 O30 2.366(6) .
Tb4 Ge2 3.4700(13) 3_667
Tb4 Tb5 3.8123(10) .
Tb4 O7 2.315(6) 3_667
Tb4 O8 2.320(6) 3_667
Tb4 O10 2.348(6) .
Tb4 O11 2.323(6) .
Tb4 O15 2.413(7) 3_667
Tb4 O21 2.384(7) .
Tb4 O27 2.509(7) .
Tb4 O4W 2.493(7) .
Tb5 Tb3 3.7259(10) 3_667
Tb5 O7 2.311(6) 3_667
Tb5 O9 2.310(6) .
Tb5 O10 2.320(6) .
Tb5 O12 2.294(6) 3_667
Tb5 O13 2.387(7) 3_667
Tb5 O20 2.418(8) .
Tb5 O31 2.527(7) 3_667
Tb5 O3W 2.618(10) .
Tb2' O18 2.567(10) 3_667
Tb2' O24 2.193(10) .
Tb2' O25 1.932(11) .
Tb2' O28 2.738(10) .
Tb2' O30 1.965(10) .
Tb2' O5W 2.469(11) .
N1 C23 1.358(13) .
N1 C27 1.331(15) .
O7 Tb4 2.315(6) 3_667
O7 Tb5 2.311(6) 3_667
O8 Tb3 2.342(6) 3_667
O8 Tb4 2.320(6) 3_667
O9 Tb3 2.308(6) 3_667
O12 Tb5 2.294(6) 3_667
O13 Tb5 2.388(7) 3_667
O13 C3 1.253(12) .
O14 Tb1 2.266(8) 4_575
O14 C3 1.256(12) .
O15 Tb4 2.413(7) 3_667
O15 C6 1.261(12) .
O16 C6 1.239(13) .
O17 Tb3 2.449(6) 3_667
O17 C9 1.269(11) .
O18 Tb2 2.477(7) 3_667
O18 Tb2' 2.567(10) 3_667
O18 C9 1.262(12) .
O19 C12 1.247(14) .
O20 C12 1.224(14) .
O21 C15 1.241(13) .
O22 C15 1.240(14) .
O23 C18 1.274(11) .
O24 C18 1.249(12) .
O25 Tb2 2.915(9) 3_566
O25 C21 1.280(14) .
O26 Tb2 2.446(8) 3_566
O26 C21 1.222(13) .
O27 C22 1.232(12) .
O28 C22 1.299(12) .
O31 Tb5 2.527(7) 3_667
O1W H1A 0.8499 .
O1W H1B 0.8501 .
O2W H2A 0.8501 .
O2W H2B 0.8500 .
O3W H3A 0.8498 .
O3W H3B 0.8499 .
O4W H4A 0.8500 .
O4W H4B 0.8500 .
O5W H5A 0.8499 .
O5W H5B 0.8499 .
C1 H1C 0.9700 .
C1 H1D 0.9700 .
C1 C2 1.536(14) .
C2 H2C 0.9700 .
C2 H2D 0.9700 .
C2 C3 1.510(13) .
C4 H4C 0.9700 .
C4 H4D 0.9700 .
C4 C5 1.526(14) .
C5 H5D 0.9700 .
C5 H5C 0.9700 .
C5 C6 1.518(14) .
C7 H7A 0.9700 .
C7 H7B 0.9700 .
C7 C8 1.542(15) .
C8 H8A 0.9700 .
C8 H8B 0.9700 .
C8 C9 1.503(14) .
C10 H10A 0.9700 .
C10 H10B 0.9700 .
C10 C11 1.526(15) .
C11 H11A 0.9700 .
C11 H11B 0.9700 .
C11 C12 1.541(18) .
C13 H13A 0.9700 .
C13 H13B 0.9700 .
C13 C14 1.549(15) .
C14 H14A 0.9700 .
C14 H14B 0.9700 .
C14 C15 1.532(16) .
C16 H16A 0.9700 .
C16 H16B 0.9700 .
C16 C17 1.535(16) .
C17 H17A 0.9700 .
C17 H17B 0.9700 .
C17 C18 1.514(15) .
C19 H19A 0.9700 .
C19 H19B 0.9700 .
C19 C20 1.468(18) .
C20 H20A 0.9700 .
C20 H20B 0.9700 .
C20 C21 1.458(19) .
C22 C23 1.470(15) .
C23 C24 1.383(16) .
C24 H24 0.9300 .
C24 C25 1.374(17) .
C25 H25 0.9300 .
C25 C26 1.401(18) .
C26 H26 0.9300 .
C26 C27 1.399(18) .
C27 H27 0.9300 .
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
Ge1 C1 C2 C3 -55.6(11) . .
Ge2 Tb1 O1 Ge1 136.9(5) . .
Ge2 Tb1 O2 Ge3 -137.9(5) . .
Ge2 Tb1 O3 Ge3 -0.1(2) . .
Ge2 Tb1 O3 Ge4 -135.1(3) . .
Ge2 Tb1 O4 Ge4 26.0(4) . .
Ge2 Tb1 O4 Ge5 -110.9(2) . .
Ge2 Tb1 O5 Ge5 108.9(3) . .
Ge2 Tb1 O5 Ge6 -29.8(4) . .
Ge2 Tb1 O6 Ge1 0.0(2) . .
Ge2 Tb1 O6 Ge6 138.6(2) . .
Ge2 Tb4 Tb5 Tb3 64.25(3) 3_667 3_667
Ge2 Tb4 Tb5 O7 -19.7(3) 3_667 3_667
Ge2 Tb4 Tb5 O9 102.50(17) 3_667 .
Ge2 Tb4 Tb5 O10 145.2(3) 3_667 .
Ge2 Tb4 Tb5 O12 25.85(16) 3_667 3_667
Ge2 Tb4 Tb5 O13 -55.6(2) 3_667 3_667
Ge2 Tb4 Tb5 O20 -178.8(2) 3_667 .
Ge2 Tb4 Tb5 O31 -140.4(9) 3_667 3_667
Ge2 Tb4 Tb5 O3W -117.6(3) 3_667 .
Ge2 Tb4 O10 Ge4 154.0(3) 3_667 .
Ge2 Tb4 O10 Tb5 -47.0(3) 3_667 .
Ge2 Tb4 O11 Ge5 168.5(3) 3_667 .
Ge2 Tb4 O11 Tb3 12.5(2) 3_667 .
Ge2 Tb4 O21 C15 58.8(12) 3_667 .
Ge2 Tb4 O27 C22 -72.5(11) 3_667 .
Ge2 C4 C5 C6 -44.4(12) . .
Ge3 C7 C8 C9 -42.2(11) . .
Ge4 C10 C11 C12 -45.8(13) . .
Ge5 Tb1 O1 Ge1 29.4(4) . .
Ge5 Tb1 O1 Ge2 -107.4(2) . .
Ge5 Tb1 O2 Ge2 110.8(2) . .
Ge5 Tb1 O2 Ge3 -27.1(4) . .
Ge5 Tb1 O3 Ge3 136.8(2) . .
Ge5 Tb1 O3 Ge4 1.8(2) . .
Ge5 Tb1 O4 Ge4 136.9(5) . .
Ge5 Tb1 O5 Ge6 -138.7(5) . .
Ge5 Tb1 O6 Ge1 -136.5(2) . .
Ge5 Tb1 O6 Ge6 2.1(2) . .
Ge5 Tb4 Tb5 Tb3 -65.00(3) . 3_667
Ge5 Tb4 Tb5 O7 -149.0(3) . 3_667
Ge5 Tb4 Tb5 O9 -26.75(17) . .
Ge5 Tb4 Tb5 O10 16.0(3) . .
Ge5 Tb4 Tb5 O12 -103.40(16) . 3_667
Ge5 Tb4 Tb5 O13 175.1(2) . 3_667
Ge5 Tb4 Tb5 O20 52.0(2) . .
Ge5 Tb4 Tb5 O31 90.3(9) . 3_667
Ge5 Tb4 Tb5 O3W 113.2(3) . .
Ge5 Tb4 O10 Ge4 37.6(4) . .
Ge5 Tb4 O10 Tb5 -163.4(3) . .
Ge5 Tb4 O11 Tb3 -156.0(5) . .
Ge5 Tb4 O21 C15 129.5(12) . .
Ge5 Tb4 O27 C22 53.8(11) . .
Ge5 C13 C14 C15 -39.0(12) . .
Ge6 Tb1 O1 Ge1 -0.6(2) . .
Ge6 Tb1 O1 Ge2 -137.5(3) . .
Ge6 Tb1 O2 Ge2 28.5(4) . .
Ge6 Tb1 O2 Ge3 -109.4(3) . .
Ge6 Tb1 O3 Ge3 110.3(2) . .
Ge6 Tb1 O3 Ge4 -24.7(4) . .
Ge6 Tb1 O4 Ge4 137.4(3) . .
Ge6 Tb1 O4 Ge5 0.5(2) . .
Ge6 Tb1 O5 Ge5 138.7(5) . .
Ge6 Tb1 O6 Ge1 -138.6(4) . .
Ge6 Tb3 Tb4 Ge2 -153.84(3) . 3_667
Ge6 Tb3 Tb4 Ge5 23.94(3) . .
Ge6 Tb3 Tb4 Tb5 -64.79(3) . .
Ge6 Tb3 Tb4 O7 -102.30(16) . 3_667
Ge6 Tb3 Tb4 O8 -139.6(3) . 3_667
Ge6 Tb3 Tb4 O10 -27.62(17) . .
Ge6 Tb3 Tb4 O11 12.0(3) . .
Ge6 Tb3 Tb4 O15 -178.35(17) . 3_667
Ge6 Tb3 Tb4 O21 46.25(17) . .
Ge6 Tb3 Tb4 O27 112.70(19) . .
Ge6 Tb3 Tb4 O4W 117.0(3) . .
Ge6 Tb3 Tb2' Ge7 69.59(11) . .
Ge6 Tb3 Tb2' Tb2 -131.3(7) . .
Ge6 Tb3 Tb2' O18 154.2(2) . 3_667
Ge6 Tb3 Tb2' O24 -29.5(3) . .
Ge6 Tb3 Tb2' O25 81.6(5) . .
Ge6 Tb3 Tb2' O28 -119.2(2) . .
Ge6 Tb3 Tb2' O30 69.0(4) . .
Ge6 Tb3 Tb2' O5W -72.0(6) . .
Ge6 Tb3 O11 Ge5 41.3(4) . .
Ge6 Tb3 O11 Tb4 -167.4(3) . .
Ge6 Tb3 O12 Tb5 -172.4(5) . 3_667
Ge6 Tb3 O23 C18 116.9(10) . .
Ge6 Tb3 O28 Tb2 78.8(2) . .
Ge6 Tb3 O28 Tb2' 75.3(2) . .
Ge6 Tb3 O28 C22 -86.2(7) . .
Ge6 Tb3 O30 Ge7 69.0(4) . .
Ge6 Tb3 O30 Tb2 -118.1(2) . .
Ge6 Tb3 O30 Tb2' -112.3(4) . .
Ge6 C16 C17 C18 -38.4(12) . .
Ge7 Tb2' O24 Tb2 -151.2(8) . .
Ge7 Tb2' O24 C18 -41.8(9) . .
Ge7 Tb2' O25 Tb2 146.8(11) . .
Ge7 Tb2' O25 Tb2 141.1(5) . 3_566
Ge7 Tb2' O25 C21 -63.6(17) . .
Ge7 Tb2' O28 Tb2 -155.7(9) . .
Ge7 Tb2' O28 Tb3 8.3(3) . .
Ge7 Tb2' O28 C22 164.9(9) . .
Ge7 Tb2' O30 Tb2 -155.3(8) . .
Ge7 Tb2' O30 Tb3 -178.9(6) . .
Ge7 Tb2' O5W Tb2 173.5(10) . .
Ge7 C19 C20 C21 5(2) . .
Tb1 Ge2 O1 Ge1 -125.2(6) . .
Tb1 Ge2 O2 Ge3 128.7(5) . .
Tb1 Ge2 O8 Tb3 -105.4(4) . 3_667
Tb1 Ge2 O8 Tb4 110.4(3) . 3_667
Tb1 Ge2 C4 C5 -96.3(8) . .
Tb1 Ge5 Tb4 Ge2 -95.78(4) . 3_667
Tb1 Ge5 Tb4 Tb3 -98.09(3) . .
Tb1 Ge5 Tb4 Tb5 20.68(3) . .
Tb1 Ge5 Tb4 O7 -2.2(2) . 3_667
Tb1 Ge5 Tb4 O8 -88.26(16) . 3_667
Tb1 Ge5 Tb4 O10 30.38(17) . .
Tb1 Ge5 Tb4 O11 -82.1(4) . .
Tb1 Ge5 Tb4 O15 -148.4(3) . 3_667
Tb1 Ge5 Tb4 O21 114.8(2) . .
Tb1 Ge5 Tb4 O27 -167.39(17) . .
Tb1 Ge5 Tb4 O4W 118.8(2) . .
Tb1 Ge5 O4 Ge4 -126.8(6) . .
Tb1 Ge5 O5 Ge6 128.6(6) . .
Tb1 Ge5 O11 Tb3 -101.1(4) . .
Tb1 Ge5 O11 Tb4 109.8(3) . .
Tb1 Ge5 C13 C14 -98.3(8) . .
Tb1 Ge6 Tb3 Tb4 19.07(3) . .
Tb1 Ge6 Tb3 Tb5 -98.84(3) . 3_667
Tb1 Ge6 Tb3 Tb2' 147.97(13) . .
Tb1 Ge6 Tb3 O8 -10.5(2) . 3_667
Tb1 Ge6 Tb3 O9 -94.63(16) . 3_667
Tb1 Ge6 Tb3 O11 26.71(18) . .
Tb1 Ge6 Tb3 O12 -93.8(3) . .
Tb1 Ge6 Tb3 O17 -153.2(4) . 3_667
Tb1 Ge6 Tb3 O23 111.2(2) . .
Tb1 Ge6 Tb3 O28 102.35(18) . .
Tb1 Ge6 Tb3 O30 173.39(17) . .
Tb1 Ge6 O5 Ge5 -127.0(6) . .
Tb1 Ge6 O6 Ge1 115.7(6) . .
Tb1 Ge6 O12 Tb3 99.3(3) . .
Tb1 Ge6 O12 Tb5 -90.6(4) . 3_667
Tb1 Ge6 C16 C17 -98.1(8) . .
Tb1 O14 C3 O13 -91.4(17) 4_575 .
Tb1 O14 C3 C2 93.7(17) 4_575 .
Tb2 Tb2' O24 C18 109.4(11) . .
Tb2 Tb2' O25 Tb2 -5.7(14) . 3_566
Tb2 Tb2' O25 C21 149.6(17) . .
Tb2 Tb2' O28 Tb3 164.0(8) . .
Tb2 Tb2' O28 C22 -39.3(13) . .
Tb2 Tb2' O30 Ge7 155.3(8) . .
Tb2 Tb2' O30 Tb3 -23.6(11) . .
Tb2 N1 C23 C22 8.7(12) . .
Tb2 N1 C23 C24 -170.5(9) . .
Tb2 N1 C27 C26 168.3(10) . .
Tb2 O18 C9 O17 -18.2(15) 3_667 .
Tb2 O18 C9 C8 160.1(8) 3_667 .
Tb2 O24 C18 O23 -29.4(15) . .
Tb2 O24 C18 C17 152.2(8) . .
Tb2 O25 C21 O26 -3.6(12) 3_566 .
Tb2 O25 C21 O26 -147.1(17) . .
Tb2 O25 C21 C20 35(3) . .
Tb2 O25 C21 C20 178.1(14) 3_566 .
Tb2 O26 C21 O25 4.5(15) 3_566 .
Tb2 O26 C21 C20 -177.3(12) 3_566 .
Tb2 O28 C22 O27 174.7(7) . .
Tb2 O28 C22 C23 -8.9(13) . .
Tb3 Ge6 Tb1 Ge2 87.19(3) . .
Tb3 Ge6 Tb1 Ge5 -46.62(3) . .
Tb3 Ge6 Tb1 O1 108.09(15) . .
Tb3 Ge6 Tb1 O2 72.3(2) . .
Tb3 Ge6 Tb1 O3 -14.2(2) . .
Tb3 Ge6 Tb1 O4 -46.95(15) . .
Tb3 Ge6 Tb1 O5 -70.9(3) . .
Tb3 Ge6 Tb1 O6 130.9(3) . .
Tb3 Ge6 Tb1 O14 -126.2(3) . 4_576
Tb3 Ge6 Tb1 O1W 30.32(18) . .
Tb3 Ge6 Tb1 O2W -170.6(3) . .
Tb3 Ge6 O5 Ge5 -9.5(4) . .
Tb3 Ge6 O5 Tb1 117.5(2) . .
Tb3 Ge6 O6 Ge1 36.0(7) . .
Tb3 Ge6 O6 Tb1 -79.7(3) . .
Tb3 Ge6 O12 Tb5 170.1(7) . 3_667
Tb3 Ge6 C16 C17 51.0(8) . .
Tb3 Tb2 Tb2' Ge7 37.0(11) . .
Tb3 Tb2 Tb2' O18 74.80(18) . 3_667
Tb3 Tb2 Tb2' O24 -79.8(4) . .
Tb3 Tb2 Tb2' O25 147.8(10) . .
Tb3 Tb2 Tb2' O28 -10.3(5) . .
Tb3 Tb2 Tb2' O30 12.8(6) . .
Tb3 Tb2 Tb2' O5W -151.2(2) . .
Tb3 Tb2 N1 C23 -24.8(8) . .
Tb3 Tb2 N1 C27 168.0(10) . .
Tb3 Tb2 O24 Tb2' 86.5(7) . .
Tb3 Tb2 O24 C18 5.6(8) . .
Tb3 Tb2 O25 Tb2 140.1(2) . 3_566
Tb3 Tb2 O25 Tb2' -34.8(11) . .
Tb3 Tb2 O25 C21 -80(2) . .
Tb3 Tb2 O28 Tb2' 16.5(8) . .
Tb3 Tb2 O28 C22 164.1(9) . .
Tb3 Tb2 O30 Ge7 173.6(6) . .
Tb3 Tb2 O30 Tb2' -158.6(10) . .
Tb3 Tb2 O5W Tb2' 71.2(7) . .
Tb3 Tb4 Tb5 Tb3 -0.17(3) . 3_667
Tb3 Tb4 Tb5 O7 -84.1(3) . 3_667
Tb3 Tb4 Tb5 O9 38.08(17) . .
Tb3 Tb4 Tb5 O10 80.8(3) . .
Tb3 Tb4 Tb5 O12 -38.57(16) . 3_667
Tb3 Tb4 Tb5 O13 -120.1(2) . 3_667
Tb3 Tb4 Tb5 O20 116.8(2) . .
Tb3 Tb4 Tb5 O31 155.2(9) . 3_667
Tb3 Tb4 Tb5 O3W 178.0(3) . .
Tb3 Tb4 O10 Ge4 85.0(4) . .
Tb3 Tb4 O10 Tb5 -116.0(2) . .
Tb3 Tb4 O11 Ge5 156.0(5) . .
Tb3 Tb4 O21 C15 100.5(11) . .
Tb3 Tb4 O27 C22 -10.4(11) . .
Tb3 Tb5 O9 Ge3 -165.7(6) 3_667 .
Tb3 Tb5 O10 Ge4 -84.9(3) 3_667 .
Tb3 Tb5 O10 Tb4 113.7(2) 3_667 .
Tb3 Tb5 O20 C12 -141(2) 3_667 .
Tb3 Tb2' O24 Tb2 -87.0(7) . .
Tb3 Tb2' O24 C18 22.4(8) . .
Tb3 Tb2' O25 Tb2 129.2(4) . 3_566
Tb3 Tb2' O25 Tb2 134.9(14) . .
Tb3 Tb2' O25 C21 -75.5(18) . .
Tb3 Tb2' O28 Tb2 -164.0(8) . .
Tb3 Tb2' O28 C22 156.7(11) . .
Tb3 Tb2' O30 Ge7 178.9(6) . .
Tb3 Tb2' O30 Tb2 23.6(11) . .
Tb3 Tb2' O5W Tb2 -63.0(7) . .
Tb3 O17 C9 O18 46.8(16) 3_667 .
Tb3 O17 C9 C8 -131.6(9) 3_667 .
Tb3 O23 C18 O24 50.7(16) . .
Tb3 O23 C18 C17 -130.8(9) . .
Tb3 O28 C22 O27 -24.2(14) . .
Tb3 O28 C22 C23 152.2(7) . .
Tb4 Ge2 Tb1 Ge5 33.16(5) 3_667 .
Tb4 Ge2 Tb1 Ge6 -26.09(4) 3_667 .
Tb4 Ge2 Tb1 O1 -71.1(3) 3_667 .
Tb4 Ge2 Tb1 O2 133.5(3) 3_667 .
Tb4 Ge2 Tb1 O3 110.66(14) 3_667 .
Tb4 Ge2 Tb1 O4 76.60(19) 3_667 .
Tb4 Ge2 Tb1 O5 -11.3(2) 3_667 .
Tb4 Ge2 Tb1 O6 -46.83(14) 3_667 .
Tb4 Ge2 Tb1 O14 179.9(2) 3_667 4_576
Tb4 Ge2 Tb1 O1W 32.30(17) 3_667 .
Tb4 Ge2 Tb1 O2W -108.2(3) 3_667 .
Tb4 Ge2 O1 Ge1 -7.1(4) 3_667 .
Tb4 Ge2 O1 Tb1 118.0(2) 3_667 .
Tb4 Ge2 O2 Ge3 55.5(5) 3_667 .
Tb4 Ge2 O2 Tb1 -73.2(3) 3_667 .
Tb4 Ge2 O8 Tb3 144.2(6) 3_667 3_667
Tb4 Ge2 C4 C5 57.6(8) 3_667 .
Tb4 Ge5 Tb1 Ge2 28.51(5) . .
Tb4 Ge5 Tb1 Ge6 108.99(4) . .
Tb4 Ge5 Tb1 O1 72.0(2) . .
Tb4 Ge5 Tb1 O2 -15.0(2) . .
Tb4 Ge5 Tb1 O3 -48.97(14) . .
Tb4 Ge5 Tb1 O4 -71.6(3) . .
Tb4 Ge5 Tb1 O5 131.9(3) . .
Tb4 Ge5 Tb1 O6 107.72(14) . .
Tb4 Ge5 Tb1 O14 -119.8(2) . 4_576
Tb4 Ge5 Tb1 O1W 29.37(16) . .
Tb4 Ge5 Tb1 O2W 168.6(3) . .
Tb4 Ge5 O4 Ge4 -8.4(4) . .
Tb4 Ge5 O4 Tb1 118.4(2) . .
Tb4 Ge5 O5 Ge6 53.3(6) . .
Tb4 Ge5 O5 Tb1 -75.3(3) . .
Tb4 Ge5 O11 Tb3 149.1(7) . .
Tb4 Ge5 C13 C14 54.4(9) . .
Tb4 Tb3 Tb2' Ge7 -177.57(4) . .
Tb4 Tb3 Tb2' Tb2 -18.4(7) . .
Tb4 Tb3 Tb2' O18 -92.9(2) . 3_667
Tb4 Tb3 Tb2' O24 83.3(3) . .
Tb4 Tb3 Tb2' O25 -165.6(5) . .
Tb4 Tb3 Tb2' O28 -6.3(3) . .
Tb4 Tb3 Tb2' O30 -178.2(4) . .
Tb4 Tb3 Tb2' O5W 40.9(7) . .
Tb4 Tb3 O11 Ge5 -151.3(6) . .
Tb4 Tb3 O12 Ge6 -75.3(3) . .
Tb4 Tb3 O12 Tb5 112.35(19) . 3_667
Tb4 Tb3 O23 C18 -145.0(10) . .
Tb4 Tb3 O28 Tb2 178.1(3) . .
Tb4 Tb3 O28 Tb2' 174.7(2) . .
Tb4 Tb3 O28 C22 13.2(7) . .
Tb4 Tb3 O30 Ge7 -175.51(14) . .
Tb4 Tb3 O30 Tb2 -2.6(5) . .
Tb4 Tb3 O30 Tb2' 3.2(6) . .
Tb4 Tb5 O9 Ge3 82.4(4) . .
Tb4 Tb5 O9 Tb3 -111.9(2) . 3_667
Tb4 Tb5 O10 Ge4 161.4(6) . .
Tb4 Tb5 O20 C12 95(2) . .
Tb4 O15 C6 O16 52.4(17) 3_667 .
Tb4 O15 C6 C5 -133.5(10) 3_667 .
Tb4 O21 C15 O22 48.8(18) . .
Tb4 O21 C15 C14 -133.4(9) . .
Tb4 O27 C22 O28 24.8(18) . .
Tb4 O27 C22 C23 -151.6(8) . .
Tb5 Tb3 Tb4 Ge2 -88.87(3) 3_667 3_667
Tb5 Tb3 Tb4 Ge5 88.91(3) 3_667 .
Tb5 Tb3 Tb4 Tb5 0.18(3) 3_667 .
Tb5 Tb3 Tb4 O7 -37.33(16) 3_667 3_667
Tb5 Tb3 Tb4 O8 -74.6(3) 3_667 3_667
Tb5 Tb3 Tb4 O10 37.35(17) 3_667 .
Tb5 Tb3 Tb4 O11 77.0(3) 3_667 .
Tb5 Tb3 Tb4 O15 -113.38(17) 3_667 3_667
Tb5 Tb3 Tb4 O21 111.22(17) 3_667 .
Tb5 Tb3 Tb4 O27 177.67(18) 3_667 .
Tb5 Tb3 Tb4 O4W -178.1(3) 3_667 .
Tb5 Tb3 Tb2' Ge7 7.05(15) 3_667 .
Tb5 Tb3 Tb2' Tb2 166.2(6) 3_667 .
Tb5 Tb3 Tb2' O18 91.7(2) 3_667 3_667
Tb5 Tb3 Tb2' O24 -92.1(3) 3_667 .
Tb5 Tb3 Tb2' O25 19.1(6) 3_667 .
Tb5 Tb3 Tb2' O28 178.3(2) 3_667 .
Tb5 Tb3 Tb2' O30 6.4(4) 3_667 .
Tb5 Tb3 Tb2' O5W -134.5(6) 3_667 .
Tb5 Tb3 O11 Ge5 89.9(4) 3_667 .
Tb5 Tb3 O11 Tb4 -118.8(2) 3_667 .
Tb5 Tb3 O12 Ge6 172.4(5) 3_667 .
Tb5 Tb3 O23 C18 90.2(10) 3_667 .
Tb5 Tb3 O28 Tb2 -1.4(7) 3_667 .
Tb5 Tb3 O28 Tb2' -4.9(7) 3_667 .
Tb5 Tb3 O28 C22 -166.4(6) 3_667 .
Tb5 Tb3 O30 Ge7 7.2(4) 3_667 .
Tb5 Tb3 O30 Tb2 -179.9(2) 3_667 .
Tb5 Tb3 O30 Tb2' -174.1(4) 3_667 .
Tb5 Tb4 O10 Ge4 -159.0(6) . .
Tb5 Tb4 O11 Ge5 -84.6(3) . .
Tb5 Tb4 O11 Tb3 119.4(2) . .
Tb5 Tb4 O21 C15 -134.1(11) . .
Tb5 Tb4 O27 C22 154.0(10) . .
Tb5 O13 C3 O14 69(2) 3_667 .
Tb5 O13 C3 C2 -115.8(14) 3_667 .
Tb5 O20 C12 O19 64(3) . .
Tb5 O20 C12 C11 -122(2) . .
Tb2' Ge7 O30 Tb2 6.9(2) . .
Tb2' Ge7 O30 Tb3 178.8(7) . .
Tb2' Ge7 O31 Tb5 -8.0(10) . 3_667
Tb2' Ge7 C19 C20 -51.8(13) . .
Tb2' Tb2 N1 C23 -110.4(13) . .
Tb2' Tb2 N1 C27 82.4(15) . .
Tb2' Tb2 O24 C18 -80.9(11) . .
Tb2' Tb2 O25 Tb2 174.9(12) . 3_566
Tb2' Tb2 O25 C21 -45(2) . .
Tb2' Tb2 O28 Tb3 -16.5(8) . .
Tb2' Tb2 O28 C22 147.6(11) . .
Tb2' Tb2 O30 Ge7 -27.8(9) . .
Tb2' Tb2 O30 Tb3 158.6(10) . .
Tb2' Tb3 Tb4 Ge2 96.04(14) . 3_667
Tb2' Tb3 Tb4 Ge5 -86.18(14) . .
Tb2' Tb3 Tb4 Tb5 -174.91(14) . .
Tb2' Tb3 Tb4 O7 147.6(2) . 3_667
Tb2' Tb3 Tb4 O8 110.3(3) . 3_667
Tb2' Tb3 Tb4 O10 -137.7(2) . .
Tb2' Tb3 Tb4 O11 -98.1(3) . .
Tb2' Tb3 Tb4 O15 71.5(2) . 3_667
Tb2' Tb3 Tb4 O21 -63.9(2) . .
Tb2' Tb3 Tb4 O27 2.6(2) . .
Tb2' Tb3 Tb4 O4W 6.8(4) . .
Tb2' Tb3 O11 Ge5 -44.5(5) . .
Tb2' Tb3 O11 Tb4 106.8(3) . .
Tb2' Tb3 O12 Ge6 67.6(3) . .
Tb2' Tb3 O12 Tb5 -104.8(2) . 3_667
Tb2' Tb3 O23 C18 -21.4(9) . .
Tb2' Tb3 O28 Tb2 3.46(17) . .
Tb2' Tb3 O28 C22 -161.5(9) . .
Tb2' Tb3 O30 Ge7 -178.7(8) . .
Tb2' Tb3 O30 Tb2 -5.8(3) . .
Tb2' O18 C9 O17 -36.1(14) 3_667 .
Tb2' O18 C9 C8 142.2(8) 3_667 .
Tb2' O24 C18 O23 -47.6(14) . .
Tb2' O24 C18 C17 134.0(9) . .
Tb2' O25 C21 O26 -163.6(12) . .
Tb2' O25 C21 C20 18(3) . .
Tb2' O28 C22 O27 -175.4(7) . .
Tb2' O28 C22 C23 1.1(15) . .
N1 Tb2 Tb2' Ge7 128.4(11) . .
N1 Tb2 Tb2' Tb3 91.4(9) . .
N1 Tb2 Tb2' O18 166.2(9) . 3_667
N1 Tb2 Tb2' O24 11.6(12) . .
N1 Tb2 Tb2' O25 -120.8(9) . .
N1 Tb2 Tb2' O28 81.0(9) . .
N1 Tb2 Tb2' O30 104.2(10) . .
N1 Tb2 Tb2' O5W -59.8(9) . .
N1 Tb2 O24 Tb2' -172.9(7) . .
N1 Tb2 O24 C18 106.2(9) . .
N1 Tb2 O25 Tb2 -69.4(6) . 3_566
N1 Tb2 O25 Tb2' 115.6(12) . .
N1 Tb2 O25 C21 70(2) . .
N1 Tb2 O28 Tb3 -154.5(4) . .
N1 Tb2 O28 Tb2' -138.0(8) . .
N1 Tb2 O28 C22 9.7(8) . .
N1 Tb2 O30 Ge7 -156.7(4) . .
N1 Tb2 O30 Tb3 29.8(4) . .
N1 Tb2 O30 Tb2' -128.8(10) . .
N1 Tb2 O5W Tb2' 147.0(7) . .
N1 C23 C24 C25 1(2) . .
O1 Ge1 O6 Ge6 -131.8(6) . .
O1 Ge1 O6 Tb1 -16.8(3) . .
O1 Ge1 O7 Tb4 -46.6(5) . 3_667
O1 Ge1 O7 Tb5 147.6(3) . 3_667
O1 Ge1 C1 C2 -138.1(7) . .
O1 Ge2 Tb1 Ge5 104.3(3) . .
O1 Ge2 Tb1 Ge6 45.0(3) . .
O1 Ge2 Tb1 O2 -155.3(4) . .
O1 Ge2 Tb1 O3 -178.2(3) . .
O1 Ge2 Tb1 O4 147.7(3) . .
O1 Ge2 Tb1 O5 59.8(4) . .
O1 Ge2 Tb1 O6 24.3(3) . .
O1 Ge2 Tb1 O14 -108.9(4) . 4_576
O1 Ge2 Tb1 O1W 103.4(3) . .
O1 Ge2 Tb1 O2W -37.0(4) . .
O1 Ge2 O2 Ge3 145.9(4) . .
O1 Ge2 O2 Tb1 17.1(3) . .
O1 Ge2 O8 Tb3 -151.2(4) . 3_667
O1 Ge2 O8 Tb4 64.6(4) . 3_667
O1 Ge2 C4 C5 -45.7(9) . .
O1 Tb1 O2 Ge2 -14.1(2) . .
O1 Tb1 O2 Ge3 -152.0(4) . .
O1 Tb1 O3 Ge3 -1.1(3) . .
O1 Tb1 O3 Ge4 -136.1(3) . .
O1 Tb1 O4 Ge4 63.7(6) . .
O1 Tb1 O4 Ge5 -73.2(5) . .
O1 Tb1 O5 Ge5 137.5(3) . .
O1 Tb1 O5 Ge6 -1.1(4) . .
O1 Tb1 O6 Ge1 14.2(2) . .
O1 Tb1 O6 Ge6 152.8(4) . .
O2 Ge2 Tb1 Ge5 -100.4(3) . .
O2 Ge2 Tb1 Ge6 -159.6(3) . .
O2 Ge2 Tb1 O1 155.3(4) . .
O2 Ge2 Tb1 O3 -22.9(3) . .
O2 Ge2 Tb1 O4 -56.9(3) . .
O2 Ge2 Tb1 O5 -144.9(4) . .
O2 Ge2 Tb1 O6 179.6(3) . .
O2 Ge2 Tb1 O14 46.4(4) . 4_576
O2 Ge2 Tb1 O1W -101.3(3) . .
O2 Ge2 Tb1 O2W 118.3(4) . .
O2 Ge2 O1 Ge1 -142.2(5) . .
O2 Ge2 O1 Tb1 -17.0(3) . .
O2 Ge2 O8 Tb3 -59.8(4) . 3_667
O2 Ge2 O8 Tb4 155.9(3) . 3_667
O2 Ge2 C4 C5 -141.7(7) . .
O2 Ge3 O3 Ge4 128.8(6) . .
O2 Ge3 O3 Tb1 16.3(3) . .
O2 Ge3 O9 Tb3 57.6(4) . 3_667
O2 Ge3 O9 Tb5 -138.1(4) . .
O2 Ge3 C7 C8 -52.1(9) . .
O2 Tb1 O1 Ge1 151.2(4) . .
O2 Tb1 O1 Ge2 14.4(2) . .
O2 Tb1 O3 Ge3 -13.9(2) . .
O2 Tb1 O3 Ge4 -148.8(4) . .
O2 Tb1 O4 Ge4 -1.7(3) . .
O2 Tb1 O4 Ge5 -138.6(3) . .
O2 Tb1 O5 Ge5 66.5(6) . .
O2 Tb1 O5 Ge6 -72.2(6) . .
O2 Tb1 O6 Ge1 0.2(3) . .
O2 Tb1 O6 Ge6 138.8(3) . .
O3 Ge3 O2 Ge2 -145.5(4) . .
O3 Ge3 O2 Tb1 -18.9(3) . .
O3 Ge3 O9 Tb3 153.6(4) . 3_667
O3 Ge3 O9 Tb5 -42.1(5) . .
O3 Ge3 C7 C8 -149.5(7) . .
O3 Ge4 O4 Ge5 145.5(5) . .
O3 Ge4 O4 Tb1 20.8(3) . .
O3 Ge4 O10 Tb4 -147.8(4) . .
O3 Ge4 O10 Tb5 54.8(5) . .
O3 Ge4 C10 C11 -38.3(10) . .
O3 Tb1 O1 Ge1 138.8(3) . .
O3 Tb1 O1 Ge2 1.9(3) . .
O3 Tb1 O2 Ge2 152.5(4) . .
O3 Tb1 O2 Ge3 14.6(2) . .
O3 Tb1 O4 Ge4 -15.8(2) . .
O3 Tb1 O4 Ge5 -152.7(4) . .
O3 Tb1 O5 Ge5 -0.9(4) . .
O3 Tb1 O5 Ge6 -139.6(3) . .
O3 Tb1 O6 Ge1 -65.9(6) . .
O3 Tb1 O6 Ge6 72.7(6) . .
O4 Ge4 O3 Ge3 -130.4(6) . .
O4 Ge4 O3 Tb1 -17.9(3) . .
O4 Ge4 O10 Tb4 -52.0(5) . .
O4 Ge4 O10 Tb5 150.7(3) . .
O4 Ge4 C10 C11 -136.3(8) . .
O4 Ge5 Tb1 Ge2 100.2(3) . .
O4 Ge5 Tb1 Ge6 -179.4(3) . .
O4 Ge5 Tb1 O1 143.6(4) . .
O4 Ge5 Tb1 O2 56.7(3) . .
O4 Ge5 Tb1 O3 22.7(3) . .
O4 Ge5 Tb1 O5 -156.5(4) . .
O4 Ge5 Tb1 O6 179.4(3) . .
O4 Ge5 Tb1 O14 -48.1(4) . 4_576
O4 Ge5 Tb1 O1W 101.0(3) . .
O4 Ge5 Tb1 O2W -119.8(4) . .
O4 Ge5 Tb4 Ge2 -138.2(2) . 3_667
O4 Ge5 Tb4 Tb3 -140.5(2) . .
O4 Ge5 Tb4 Tb5 -21.7(2) . .
O4 Ge5 Tb4 O7 -44.6(3) . 3_667
O4 Ge5 Tb4 O8 -130.7(3) . 3_667
O4 Ge5 Tb4 O10 -12.0(3) . .
O4 Ge5 Tb4 O11 -124.5(4) . .
O4 Ge5 Tb4 O15 169.2(4) . 3_667
O4 Ge5 Tb4 O21 72.4(3) . .
O4 Ge5 Tb4 O27 150.2(3) . .
O4 Ge5 Tb4 O4W 76.4(3) . .
O4 Ge5 O5 Ge6 145.1(5) . .
O4 Ge5 O5 Tb1 16.5(3) . .
O4 Ge5 O11 Tb3 -147.6(4) . .
O4 Ge5 O11 Tb4 63.2(4) . .
O4 Ge5 C13 C14 -48.7(9) . .
O4 Tb1 O1 Ge1 73.3(5) . .
O4 Tb1 O1 Ge2 -63.5(6) . .
O4 Tb1 O2 Ge2 138.3(3) . .
O4 Tb1 O2 Ge3 0.5(4) . .
O4 Tb1 O3 Ge3 150.5(4) . .
O4 Tb1 O3 Ge4 15.5(2) . .
O4 Tb1 O5 Ge5 -13.6(2) . .
O4 Tb1 O5 Ge6 -152.3(4) . .
O4 Tb1 O6 Ge1 -136.2(3) . .
O4 Tb1 O6 Ge6 2.4(4) . .
O5 Ge5 Tb1 Ge2 -103.4(3) . .
O5 Ge5 Tb1 Ge6 -22.9(3) . .
O5 Ge5 Tb1 O1 -59.9(4) . .
O5 Ge5 Tb1 O2 -146.8(4) . .
O5 Ge5 Tb1 O3 179.2(3) . .
O5 Ge5 Tb1 O4 156.5(4) . .
O5 Ge5 Tb1 O6 -24.1(3) . .
O5 Ge5 Tb1 O14 108.4(4) . 4_576
O5 Ge5 Tb1 O1W -102.5(3) . .
O5 Ge5 Tb1 O2W 36.7(4) . .
O5 Ge5 Tb4 Ge2 -49.2(3) . 3_667
O5 Ge5 Tb4 Tb3 -51.5(3) . .
O5 Ge5 Tb4 Tb5 67.3(3) . .
O5 Ge5 Tb4 O7 44.3(3) . 3_667
O5 Ge5 Tb4 O8 -41.7(3) . 3_667
O5 Ge5 Tb4 O10 77.0(3) . .
O5 Ge5 Tb4 O11 -35.5(4) . .
O5 Ge5 Tb4 O15 -101.8(4) . 3_667
O5 Ge5 Tb4 O21 161.4(4) . .
O5 Ge5 Tb4 O27 -120.8(3) . .
O5 Ge5 Tb4 O4W 165.4(3) . .
O5 Ge5 O4 Ge4 -142.9(5) . .
O5 Ge5 O4 Tb1 -16.1(3) . .
O5 Ge5 O11 Tb3 -55.9(5) . .
O5 Ge5 O11 Tb4 155.0(3) . .
O5 Ge5 C13 C14 -144.7(8) . .
O5 Ge6 Tb1 Ge2 158.1(3) . .
O5 Ge6 Tb1 Ge5 24.3(3) . .
O5 Ge6 Tb1 O1 179.0(3) . .
O5 Ge6 Tb1 O2 143.2(4) . .
O5 Ge6 Tb1 O3 56.7(4) . .
O5 Ge6 Tb1 O4 23.9(3) . .
O5 Ge6 Tb1 O6 -158.2(4) . .
O5 Ge6 Tb1 O14 -55.3(4) . 4_576
O5 Ge6 Tb1 O1W 101.2(4) . .
O5 Ge6 Tb1 O2W -99.8(4) . .
O5 Ge6 Tb3 Tb4 -19.9(2) . .
O5 Ge6 Tb3 Tb5 -137.8(2) . 3_667
O5 Ge6 Tb3 Tb2' 109.0(2) . .
O5 Ge6 Tb3 O8 -49.4(3) . 3_667
O5 Ge6 Tb3 O9 -133.6(3) . 3_667
O5 Ge6 Tb3 O11 -12.3(3) . .
O5 Ge6 Tb3 O12 -132.8(4) . .
O5 Ge6 Tb3 O17 167.9(4) . 3_667
O5 Ge6 Tb3 O23 72.2(3) . .
O5 Ge6 Tb3 O28 63.4(3) . .
O5 Ge6 Tb3 O30 134.4(3) . .
O5 Ge6 O6 Ge1 130.0(6) . .
O5 Ge6 O6 Tb1 14.3(3) . .
O5 Ge6 O12 Tb3 54.7(4) . .
O5 Ge6 O12 Tb5 -135.2(4) . 3_667
O5 Ge6 C16 C17 -53.0(9) . .
O5 Tb1 O1 Ge1 -0.1(4) . .
O5 Tb1 O1 Ge2 -136.9(3) . .
O5 Tb1 O2 Ge2 70.5(6) . .
O5 Tb1 O2 Ge3 -67.3(6) . .
O5 Tb1 O3 Ge3 137.3(3) . .
O5 Tb1 O3 Ge4 2.3(4) . .
O5 Tb1 O4 Ge4 150.6(4) . .
O5 Tb1 O4 Ge5 13.7(2) . .
O5 Tb1 O6 Ge1 -150.8(4) . .
O5 Tb1 O6 Ge6 -12.2(2) . .
O6 Ge1 O1 Ge2 142.8(5) . .
O6 Ge1 O1 Tb1 18.5(3) . .
O6 Ge1 O7 Tb4 -144.5(4) . 3_667
O6 Ge1 O7 Tb5 49.7(5) . 3_667
O6 Ge1 C1 C2 -37.4(8) . .
O6 Ge6 Tb1 Ge2 -43.7(3) . .
O6 Ge6 Tb1 Ge5 -177.5(3) . .
O6 Ge6 Tb1 O1 -22.8(3) . .
O6 Ge6 Tb1 O2 -58.6(4) . .
O6 Ge6 Tb1 O3 -145.1(4) . .
O6 Ge6 Tb1 O4 -177.8(3) . .
O6 Ge6 Tb1 O5 158.2(4) . .
O6 Ge6 Tb1 O14 102.9(4) . 4_576
O6 Ge6 Tb1 O1W -100.6(3) . .
O6 Ge6 Tb1 O2W 58.5(4) . .
O6 Ge6 Tb3 Tb4 72.5(3) . .
O6 Ge6 Tb3 Tb5 -45.4(3) . 3_667
O6 Ge6 Tb3 Tb2' -158.6(3) . .
O6 Ge6 Tb3 O8 43.0(4) . 3_667
O6 Ge6 Tb3 O9 -41.2(3) . 3_667
O6 Ge6 Tb3 O11 80.1(3) . .
O6 Ge6 Tb3 O12 -40.4(5) . .
O6 Ge6 Tb3 O17 -99.7(5) . 3_667
O6 Ge6 Tb3 O23 164.6(4) . .
O6 Ge6 Tb3 O28 155.8(3) . .
O6 Ge6 Tb3 O30 -133.2(3) . .
O6 Ge6 O5 Ge5 -143.5(5) . .
O6 Ge6 O5 Tb1 -16.5(3) . .
O6 Ge6 O12 Tb3 151.3(3) . .
O6 Ge6 O12 Tb5 -38.6(5) . 3_667
O6 Ge6 C16 C17 -150.6(7) . .
O6 Tb1 O1 Ge1 -14.2(2) . .
O6 Tb1 O1 Ge2 -151.0(4) . .
O6 Tb1 O2 Ge2 -0.4(4) . .
O6 Tb1 O2 Ge3 -138.3(3) . .
O6 Tb1 O3 Ge3 65.8(6) . .
O6 Tb1 O3 Ge4 -69.2(6) . .
O6 Tb1 O4 Ge4 136.2(3) . .
O6 Tb1 O4 Ge5 -0.7(4) . .
O6 Tb1 O5 Ge5 151.5(4) . .
O6 Tb1 O5 Ge6 12.8(2) . .
O7 Ge1 O1 Ge2 28.1(6) . .
O7 Ge1 O1 Tb1 -96.3(3) . .
O7 Ge1 O6 Ge6 -22.3(7) . .
O7 Ge1 O6 Tb1 92.7(3) . .
O7 Ge1 C1 C2 95.6(8) . .
O7 Tb4 Tb5 Tb3 84.0(3) 3_667 3_667
O7 Tb4 Tb5 O9 122.2(3) 3_667 .
O7 Tb4 Tb5 O10 164.9(4) 3_667 .
O7 Tb4 Tb5 O12 45.6(3) 3_667 3_667
O7 Tb4 Tb5 O13 -35.9(3) 3_667 3_667
O7 Tb4 Tb5 O20 -159.1(4) 3_667 .
O7 Tb4 Tb5 O31 -120.7(10) 3_667 3_667
O7 Tb4 Tb5 O3W -97.9(4) 3_667 .
O7 Tb4 O10 Ge4 -168.1(5) 3_667 .
O7 Tb4 O10 Tb5 -9.1(2) 3_667 .
O7 Tb4 O11 Ge5 -119.3(3) 3_667 .
O7 Tb4 O11 Tb3 84.7(3) 3_667 .
O7 Tb4 O21 C15 -123.1(10) 3_667 .
O7 Tb4 O27 C22 -105.0(11) 3_667 .
O7 Tb5 O9 Ge3 117.4(4) 3_667 .
O7 Tb5 O9 Tb3 -76.9(3) 3_667 3_667
O7 Tb5 O10 Ge4 170.5(4) 3_667 .
O7 Tb5 O10 Tb4 9.1(2) 3_667 .
O7 Tb5 O20 C12 79(2) 3_667 .
O8 Ge2 Tb1 Ge5 -3.76(19) . .
O8 Ge2 Tb1 Ge6 -63.01(19) . .
O8 Ge2 Tb1 O1 -108.0(3) . .
O8 Ge2 Tb1 O2 96.6(3) . .
O8 Ge2 Tb1 O3 73.7(2) . .
O8 Ge2 Tb1 O4 39.7(3) . .
O8 Ge2 Tb1 O5 -48.3(3) . .
O8 Ge2 Tb1 O6 -83.8(2) . .
O8 Ge2 Tb1 O14 143.0(3) . 4_576
O8 Ge2 Tb1 O1W -4.6(2) . .
O8 Ge2 Tb1 O2W -145.1(3) . .
O8 Ge2 O1 Ge1 -39.8(5) . .
O8 Ge2 O1 Tb1 85.3(3) . .
O8 Ge2 O2 Ge3 35.3(5) . .
O8 Ge2 O2 Tb1 -93.4(3) . .
O8 Ge2 C4 C5 96.5(8) . .
O8 Tb3 Tb4 Ge2 -14.3(3) 3_667 3_667
O8 Tb3 Tb4 Ge5 163.5(3) 3_667 .
O8 Tb3 Tb4 Tb5 74.8(3) 3_667 .
O8 Tb3 Tb4 O7 37.3(3) 3_667 3_667
O8 Tb3 Tb4 O10 112.0(3) 3_667 .
O8 Tb3 Tb4 O11 151.6(4) 3_667 .
O8 Tb3 Tb4 O15 -38.8(3) 3_667 3_667
O8 Tb3 Tb4 O21 -174.2(3) 3_667 .
O8 Tb3 Tb4 O27 -107.7(3) 3_667 .
O8 Tb3 Tb4 O4W -103.5(4) 3_667 .
O8 Tb3 Tb2' Ge7 -132.0(2) 3_667 .
O8 Tb3 Tb2' Tb2 27.1(8) 3_667 .
O8 Tb3 Tb2' O18 -47.4(3) 3_667 3_667
O8 Tb3 Tb2' O24 128.8(3) 3_667 .
O8 Tb3 Tb2' O25 -120.0(5) 3_667 .
O8 Tb3 Tb2' O28 39.2(3) 3_667 .
O8 Tb3 Tb2' O30 -132.6(4) 3_667 .
O8 Tb3 Tb2' O5W 86.4(6) 3_667 .
O8 Tb3 O11 Ge5 -168.7(5) 3_667 .
O8 Tb3 O11 Tb4 -17.4(2) 3_667 .
O8 Tb3 O12 Ge6 -114.8(3) 3_667 .
O8 Tb3 O12 Tb5 72.8(3) 3_667 3_667
O8 Tb3 O23 C18 -140.8(9) 3_667 .
O8 Tb3 O28 Tb2 -147.1(3) 3_667 .
O8 Tb3 O28 Tb2' -150.6(3) 3_667 .
O8 Tb3 O28 C22 47.9(7) 3_667 .
O8 Tb3 O30 Ge7 -106.0(5) 3_667 .
O8 Tb3 O30 Tb2 66.9(4) 3_667 .
O8 Tb3 O30 Tb2' 72.7(6) 3_667 .
O8 Tb4 Tb5 Tb3 36.77(16) 3_667 3_667
O8 Tb4 Tb5 O7 -47.2(3) 3_667 3_667
O8 Tb4 Tb5 O9 75.0(2) 3_667 .
O8 Tb4 Tb5 O10 117.8(3) 3_667 .
O8 Tb4 Tb5 O12 -1.6(2) 3_667 3_667
O8 Tb4 Tb5 O13 -83.1(3) 3_667 3_667
O8 Tb4 Tb5 O20 153.8(3) 3_667 .
O8 Tb4 Tb5 O31 -167.9(9) 3_667 3_667
O8 Tb4 Tb5 O3W -145.0(3) 3_667 .
O8 Tb4 O10 Ge4 124.4(4) 3_667 .
O8 Tb4 O10 Tb5 -76.6(3) 3_667 .
O8 Tb4 O11 Ge5 173.5(4) 3_667 .
O8 Tb4 O11 Tb3 17.5(2) 3_667 .
O8 Tb4 O21 C15 95.5(11) 3_667 .
O8 Tb4 O27 C22 -45.5(11) 3_667 .
O9 Ge3 O2 Ge2 -39.2(5) . .
O9 Ge3 O2 Tb1 87.4(3) . .
O9 Ge3 O3 Ge4 14.0(6) . .
O9 Ge3 O3 Tb1 -98.5(3) . .
O9 Ge3 C7 C8 88.8(8) . .
O9 Tb3 Tb4 Ge2 -49.96(16) 3_667 3_667
O9 Tb3 Tb4 Ge5 127.82(16) 3_667 .
O9 Tb3 Tb4 Tb5 39.09(16) 3_667 .
O9 Tb3 Tb4 O7 1.6(2) 3_667 3_667
O9 Tb3 Tb4 O8 -35.7(3) 3_667 3_667
O9 Tb3 Tb4 O10 76.3(2) 3_667 .
O9 Tb3 Tb4 O11 115.9(3) 3_667 .
O9 Tb3 Tb4 O15 -74.5(2) 3_667 3_667
O9 Tb3 Tb4 O21 150.1(2) 3_667 .
O9 Tb3 Tb4 O27 -143.4(2) 3_667 .
O9 Tb3 Tb4 O4W -139.2(4) 3_667 .
O9 Tb3 Tb2' Ge7 -33.0(2) 3_667 .
O9 Tb3 Tb2' Tb2 126.1(7) 3_667 .
O9 Tb3 Tb2' O18 51.6(3) 3_667 3_667
O9 Tb3 Tb2' O24 -132.1(3) 3_667 .
O9 Tb3 Tb2' O25 -21.0(6) 3_667 .
O9 Tb3 Tb2' O28 138.2(3) 3_667 .
O9 Tb3 Tb2' O30 -33.6(5) 3_667 .
O9 Tb3 Tb2' O5W -174.6(6) 3_667 .
O9 Tb3 O11 Ge5 126.7(4) 3_667 .
O9 Tb3 O11 Tb4 -82.0(3) 3_667 .
O9 Tb3 O12 Ge6 179.1(4) 3_667 .
O9 Tb3 O12 Tb5 6.8(2) 3_667 3_667
O9 Tb3 O23 C18 78.5(10) 3_667 .
O9 Tb3 O28 Tb2 -73.3(4) 3_667 .
O9 Tb3 O28 Tb2' -76.7(4) 3_667 .
O9 Tb3 O28 C22 121.8(7) 3_667 .
O9 Tb3 O30 Ge7 -28.7(5) 3_667 .
O9 Tb3 O30 Tb2 144.3(3) 3_667 .
O9 Tb3 O30 Tb2' 150.0(4) 3_667 .
O9 Tb5 O10 Ge4 -59.2(4) . .
O9 Tb5 O10 Tb4 139.4(3) . .
O9 Tb5 O20 C12 -159(2) . .
O10 Ge4 O3 Ge3 -24.0(7) . .
O10 Ge4 O3 Tb1 88.5(3) . .
O10 Ge4 O4 Ge5 31.0(5) . .
O10 Ge4 O4 Tb1 -93.7(3) . .
O10 Ge4 C10 C11 97.5(9) . .
O10 Tb4 Tb5 Tb3 -81.0(3) . 3_667
O10 Tb4 Tb5 O7 -164.9(4) . 3_667
O10 Tb4 Tb5 O9 -42.7(3) . .
O10 Tb4 Tb5 O12 -119.4(3) . 3_667
O10 Tb4 Tb5 O13 159.1(3) . 3_667
O10 Tb4 Tb5 O20 36.0(4) . .
O10 Tb4 Tb5 O31 74.4(10) . 3_667
O10 Tb4 Tb5 O3W 97.2(4) . .
O10 Tb4 O11 Ge5 -61.2(3) . .
O10 Tb4 O11 Tb3 142.8(3) . .
O10 Tb4 O21 C15 -151.0(11) . .
O10 Tb4 O27 C22 82.4(12) . .
O10 Tb5 O9 Ge3 58.9(4) . .
O10 Tb5 O9 Tb3 -135.4(3) . 3_667
O10 Tb5 O20 C12 116(2) . .
O11 Ge5 Tb1 Ge2 -9.2(2) . .
O11 Ge5 Tb1 Ge6 71.3(2) . .
O11 Ge5 Tb1 O1 34.3(3) . .
O11 Ge5 Tb1 O2 -52.7(3) . .
O11 Ge5 Tb1 O3 -86.7(2) . .
O11 Ge5 Tb1 O4 -109.3(4) . .
O11 Ge5 Tb1 O5 94.2(4) . .
O11 Ge5 Tb1 O6 70.0(2) . .
O11 Ge5 Tb1 O14 -157.5(3) . 4_576
O11 Ge5 Tb1 O1W -8.3(3) . .
O11 Ge5 Tb1 O2W 130.9(3) . .
O11 Ge5 Tb4 Ge2 -13.7(4) . 3_667
O11 Ge5 Tb4 Tb3 -16.0(4) . .
O11 Ge5 Tb4 Tb5 102.8(4) . .
O11 Ge5 Tb4 O7 79.9(4) . 3_667
O11 Ge5 Tb4 O8 -6.2(4) . 3_667
O11 Ge5 Tb4 O10 112.5(4) . .
O11 Ge5 Tb4 O15 -66.3(5) . 3_667
O11 Ge5 Tb4 O21 -163.1(4) . .
O11 Ge5 Tb4 O27 -85.3(4) . .
O11 Ge5 Tb4 O4W -159.1(4) . .
O11 Ge5 O4 Ge4 -40.9(6) . .
O11 Ge5 O4 Tb1 85.9(3) . .
O11 Ge5 O5 Ge6 32.3(5) . .
O11 Ge5 O5 Tb1 -96.3(3) . .
O11 Ge5 C13 C14 93.3(8) . .
O11 Tb3 Tb4 Ge2 -165.9(3) . 3_667
O11 Tb3 Tb4 Ge5 11.9(3) . .
O11 Tb3 Tb4 Tb5 -76.8(3) . .
O11 Tb3 Tb4 O7 -114.3(3) . 3_667
O11 Tb3 Tb4 O8 -151.6(4) . 3_667
O11 Tb3 Tb4 O10 -39.6(3) . .
O11 Tb3 Tb4 O15 169.6(3) . 3_667
O11 Tb3 Tb4 O21 34.2(3) . .
O11 Tb3 Tb4 O27 100.7(3) . .
O11 Tb3 Tb4 O4W 105.0(4) . .
O11 Tb3 Tb2' Ge7 138.71(19) . .
O11 Tb3 Tb2' Tb2 -62.2(7) . .
O11 Tb3 Tb2' O18 -136.7(3) . 3_667
O11 Tb3 Tb2' O24 39.6(4) . .
O11 Tb3 Tb2' O25 150.7(5) . .
O11 Tb3 Tb2' O28 -50.1(3) . .
O11 Tb3 Tb2' O30 138.1(4) . .
O11 Tb3 Tb2' O5W -2.8(7) . .
O11 Tb3 O12 Ge6 -53.7(3) . .
O11 Tb3 O12 Tb5 133.9(3) . 3_667
O11 Tb3 O23 C18 -165.1(10) . .
O11 Tb3 O28 Tb2 142.8(3) . .
O11 Tb3 O28 Tb2' 139.4(3) . .
O11 Tb3 O28 C22 -22.1(7) . .
O11 Tb3 O30 Ge7 120.6(4) . .
O11 Tb3 O30 Tb2 -66.5(4) . .
O11 Tb3 O30 Tb2' -60.7(6) . .
O11 Tb4 Tb5 Tb3 -37.74(16) . 3_667
O11 Tb4 Tb5 O7 -121.7(3) . 3_667
O11 Tb4 Tb5 O9 0.5(2) . .
O11 Tb4 Tb5 O10 43.2(3) . .
O11 Tb4 Tb5 O12 -76.1(2) . 3_667
O11 Tb4 Tb5 O13 -157.6(3) . 3_667
O11 Tb4 Tb5 O20 79.2(3) . .
O11 Tb4 Tb5 O31 117.6(9) . 3_667
O11 Tb4 Tb5 O3W 140.4(3) . .
O11 Tb4 O10 Ge4 62.3(4) . .
O11 Tb4 O10 Tb5 -138.6(3) . .
O11 Tb4 O21 C15 121.5(11) . .
O11 Tb4 O27 C22 26.6(11) . .
O12 Ge6 Tb1 Ge2 49.3(2) . .
O12 Ge6 Tb1 Ge5 -84.5(2) . .
O12 Ge6 Tb1 O1 70.2(3) . .
O12 Ge6 Tb1 O2 34.4(3) . .
O12 Ge6 Tb1 O3 -52.0(3) . .
O12 Ge6 Tb1 O4 -84.8(3) . .
O12 Ge6 Tb1 O5 -108.8(4) . .
O12 Ge6 Tb1 O6 93.0(4) . .
O12 Ge6 Tb1 O14 -164.1(4) . 4_576
O12 Ge6 Tb1 O1W -7.6(3) . .
O12 Ge6 Tb1 O2W 151.5(4) . .
O12 Ge6 Tb3 Tb4 112.9(3) . .
O12 Ge6 Tb3 Tb5 -5.1(3) . 3_667
O12 Ge6 Tb3 Tb2' -118.2(4) . .
O12 Ge6 Tb3 O8 83.3(4) . 3_667
O12 Ge6 Tb3 O9 -0.8(4) . 3_667
O12 Ge6 Tb3 O11 120.5(4) . .
O12 Ge6 Tb3 O17 -59.4(5) . 3_667
O12 Ge6 Tb3 O23 -155.0(4) . .
O12 Ge6 Tb3 O28 -163.9(4) . .
O12 Ge6 Tb3 O30 -92.8(4) . .
O12 Ge6 O5 Ge5 -38.0(6) . .
O12 Ge6 O5 Tb1 89.0(3) . .
O12 Ge6 O6 Ge1 13.1(6) . .
O12 Ge6 O6 Tb1 -102.6(3) . .
O12 Ge6 C16 C17 90.1(8) . .
O12 Tb3 Tb4 Ge2 -127.88(17) . 3_667
O12 Tb3 Tb4 Ge5 49.90(17) . .
O12 Tb3 Tb4 Tb5 -38.83(17) . .
O12 Tb3 Tb4 O7 -76.3(2) . 3_667
O12 Tb3 Tb4 O8 -113.6(3) . 3_667
O12 Tb3 Tb4 O10 -1.7(2) . .
O12 Tb3 Tb4 O11 38.0(3) . .
O12 Tb3 Tb4 O15 -152.4(2) . 3_667
O12 Tb3 Tb4 O21 72.2(2) . .
O12 Tb3 Tb4 O27 138.7(3) . .
O12 Tb3 Tb4 O4W 142.9(4) . .
O12 Tb3 Tb2' Ge7 45.3(2) . .
O12 Tb3 Tb2' Tb2 -155.5(7) . .
O12 Tb3 Tb2' O18 130.0(3) . 3_667
O12 Tb3 Tb2' O24 -53.8(4) . .
O12 Tb3 Tb2' O25 57.3(6) . .
O12 Tb3 Tb2' O28 -143.4(3) . .
O12 Tb3 Tb2' O30 44.7(5) . .
O12 Tb3 Tb2' O5W -96.2(6) . .
O12 Tb3 O11 Ge5 63.8(4) . .
O12 Tb3 O11 Tb4 -144.9(3) . .
O12 Tb3 O23 C18 105.4(10) . .
O12 Tb3 O28 Tb2 67.5(4) . .
O12 Tb3 O28 Tb2' 64.0(4) . .
O12 Tb3 O28 C22 -97.5(8) . .
O12 Tb3 O30 Ge7 42.9(5) . .
O12 Tb3 O30 Tb2 -144.2(3) . .
O12 Tb3 O30 Tb2' -138.4(4) . .
O12 Tb5 O9 Ge3 -172.4(5) 3_667 .
O12 Tb5 O9 Tb3 -6.7(2) 3_667 3_667
O12 Tb5 O10 Ge4 -121.0(3) 3_667 .
O12 Tb5 O10 Tb4 77.5(3) 3_667 .
O12 Tb5 O20 C12 -124(2) 3_667 .
O13 Tb5 O9 Ge3 -133.9(4) 3_667 .
O13 Tb5 O9 Tb3 31.7(5) 3_667 3_667
O13 Tb5 O10 Ge4 132.0(4) 3_667 .
O13 Tb5 O10 Tb4 -29.5(5) 3_667 .
O13 Tb5 O20 C12 -17(2) 3_667 .
O14 Tb1 O1 Ge1 -137.6(3) 4_576 .
O14 Tb1 O1 Ge2 85.5(4) 4_576 .
O14 Tb1 O2 Ge2 -138.0(3) 4_576 .
O14 Tb1 O2 Ge3 84.2(3) 4_576 .
O14 Tb1 O3 Ge3 -115.3(4) 4_576 .
O14 Tb1 O3 Ge4 109.7(4) 4_576 .
O14 Tb1 O4 Ge4 -89.3(3) 4_576 .
O14 Tb1 O4 Ge5 133.8(3) 4_576 .
O14 Tb1 O5 Ge5 -82.4(4) 4_576 .
O14 Tb1 O5 Ge6 138.9(3) 4_576 .
O14 Tb1 O6 Ge1 115.6(4) 4_576 .
O14 Tb1 O6 Ge6 -105.8(4) 4_576 .
O15 Tb4 Tb5 Tb3 109.49(17) 3_667 3_667
O15 Tb4 Tb5 O7 25.5(3) 3_667 3_667
O15 Tb4 Tb5 O9 147.7(2) 3_667 .
O15 Tb4 Tb5 O10 -169.5(3) 3_667 .
O15 Tb4 Tb5 O12 71.1(2) 3_667 3_667
O15 Tb4 Tb5 O13 -10.4(3) 3_667 3_667
O15 Tb4 Tb5 O20 -133.5(3) 3_667 .
O15 Tb4 Tb5 O31 -95.2(9) 3_667 3_667
O15 Tb4 Tb5 O3W -72.3(3) 3_667 .
O15 Tb4 O10 Ge4 -143.3(4) 3_667 .
O15 Tb4 O10 Tb5 15.7(5) 3_667 .
O15 Tb4 O11 Ge5 141.7(3) 3_667 .
O15 Tb4 O11 Tb3 -14.3(4) 3_667 .
O15 Tb4 O21 C15 -9.6(12) 3_667 .
O15 Tb4 O27 C22 -116.7(11) 3_667 .
O17 Tb3 Tb4 Ge2 22.66(17) 3_667 3_667
O17 Tb3 Tb4 Ge5 -159.56(17) 3_667 .
O17 Tb3 Tb4 Tb5 111.71(17) 3_667 .
O17 Tb3 Tb4 O7 74.2(2) 3_667 3_667
O17 Tb3 Tb4 O8 36.9(3) 3_667 3_667
O17 Tb3 Tb4 O10 148.9(2) 3_667 .
O17 Tb3 Tb4 O11 -171.5(3) 3_667 .
O17 Tb3 Tb4 O15 -1.8(2) 3_667 3_667
O17 Tb3 Tb4 O21 -137.2(2) 3_667 .
O17 Tb3 Tb4 O27 -70.8(2) 3_667 .
O17 Tb3 Tb4 O4W -66.5(4) 3_667 .
O17 Tb3 Tb2' Ge7 -86.6(2) 3_667 .
O17 Tb3 Tb2' Tb2 72.5(7) 3_667 .
O17 Tb3 Tb2' O18 -2.0(3) 3_667 3_667
O17 Tb3 Tb2' O24 174.2(4) 3_667 .
O17 Tb3 Tb2' O25 -74.6(6) 3_667 .
O17 Tb3 Tb2' O28 84.6(3) 3_667 .
O17 Tb3 Tb2' O30 -87.3(4) 3_667 .
O17 Tb3 Tb2' O5W 131.8(7) 3_667 .
O17 Tb3 O11 Ge5 -138.8(4) 3_667 .
O17 Tb3 O11 Tb4 12.5(5) 3_667 .
O17 Tb3 O12 Ge6 147.6(3) 3_667 .
O17 Tb3 O12 Tb5 -24.8(4) 3_667 3_667
O17 Tb3 O23 C18 -26.7(11) 3_667 .
O17 Tb3 O28 Tb2 -74.6(3) 3_667 .
O17 Tb3 O28 Tb2' -78.1(3) 3_667 .
O17 Tb3 O28 C22 120.4(8) 3_667 .
O17 Tb3 O30 Ge7 -96.1(5) 3_667 .
O17 Tb3 O30 Tb2 76.8(3) 3_667 .
O17 Tb3 O30 Tb2' 82.6(4) 3_667 .
O18 Tb2 Tb2' Ge7 -37.8(12) 3_667 .
O18 Tb2 Tb2' Tb3 -74.80(18) 3_667 .
O18 Tb2 Tb2' O24 -154.6(4) 3_667 .
O18 Tb2 Tb2' O25 73.0(9) 3_667 .
O18 Tb2 Tb2' O28 -85.1(5) 3_667 .
O18 Tb2 Tb2' O30 -62.0(7) 3_667 .
O18 Tb2 Tb2' O5W 134.0(2) 3_667 .
O18 Tb2 N1 C23 52.6(8) 3_667 .
O18 Tb2 N1 C27 -114.7(10) 3_667 .
O18 Tb2 O24 Tb2' 46.8(8) 3_667 .
O18 Tb2 O24 C18 -34.1(11) 3_667 .
O18 Tb2 O25 Tb2 71.2(3) 3_667 3_566
O18 Tb2 O25 Tb2' -103.7(12) 3_667 .
O18 Tb2 O25 C21 -149(2) 3_667 .
O18 Tb2 O28 Tb3 71.5(3) 3_667 .
O18 Tb2 O28 Tb2' 88.0(8) 3_667 .
O18 Tb2 O28 C22 -124.4(8) 3_667 .
O18 Tb2 O30 Ge7 82.8(4) 3_667 .
O18 Tb2 O30 Tb3 -90.8(3) 3_667 .
O18 Tb2 O30 Tb2' 110.6(9) 3_667 .
O18 Tb2 O5W Tb2' -90.1(7) 3_667 .
O18 Tb2' O24 Tb2 -78.3(11) 3_667 .
O18 Tb2' O24 C18 31.0(16) 3_667 .
O18 Tb2' O25 Tb2 67.5(11) 3_667 .
O18 Tb2' O25 Tb2 61.8(5) 3_667 3_566
O18 Tb2' O25 C21 -142.9(17) 3_667 .
O18 Tb2' O28 Tb2 -81.3(8) 3_667 .
O18 Tb2' O28 Tb3 82.7(3) 3_667 .
O18 Tb2' O28 C22 -120.7(10) 3_667 .
O18 Tb2' O30 Ge7 93.5(4) 3_667 .
O18 Tb2' O30 Tb2 -61.9(9) 3_667 .
O18 Tb2' O30 Tb3 -85.5(4) 3_667 .
O18 Tb2' O5W Tb2 58.3(6) 3_667 .
O20 Tb5 O9 Ge3 -15.0(4) . .
O20 Tb5 O9 Tb3 150.6(3) . 3_667
O20 Tb5 O10 Ge4 18.6(4) . .
O20 Tb5 O10 Tb4 -142.8(4) . .
O21 Tb4 Tb5 Tb3 -109.77(17) . 3_667
O21 Tb4 Tb5 O7 166.3(3) . 3_667
O21 Tb4 Tb5 O9 -71.5(2) . .
O21 Tb4 Tb5 O10 -28.8(3) . .
O21 Tb4 Tb5 O12 -148.2(2) . 3_667
O21 Tb4 Tb5 O13 130.3(3) . 3_667
O21 Tb4 Tb5 O20 7.2(3) . .
O21 Tb4 Tb5 O31 45.6(9) . 3_667
O21 Tb4 Tb5 O3W 68.4(3) . .
O21 Tb4 O10 Ge4 -8.7(4) . .
O21 Tb4 O10 Tb5 150.3(3) . .
O21 Tb4 O11 Ge5 12.3(3) . .
O21 Tb4 O11 Tb3 -143.7(3) . .
O21 Tb4 O27 C22 98.7(11) . .
O23 Tb3 Tb4 Ge2 160.90(16) . 3_667
O23 Tb3 Tb4 Ge5 -21.32(16) . .
O23 Tb3 Tb4 Tb5 -110.05(17) . .
O23 Tb3 Tb4 O7 -147.6(2) . 3_667
O23 Tb3 Tb4 O8 175.2(3) . 3_667
O23 Tb3 Tb4 O10 -72.9(2) . .
O23 Tb3 Tb4 O11 -33.2(3) . .
O23 Tb3 Tb4 O15 136.4(2) . 3_667
O23 Tb3 Tb4 O21 1.0(2) . .
O23 Tb3 Tb4 O27 67.4(2) . .
O23 Tb3 Tb4 O4W 71.7(4) . .
O23 Tb3 Tb2' Ge7 97.5(2) . .
O23 Tb3 Tb2' Tb2 -103.4(7) . .
O23 Tb3 Tb2' O18 -177.9(3) . 3_667
O23 Tb3 Tb2' O24 -1.6(3) . .
O23 Tb3 Tb2' O25 109.5(6) . .
O23 Tb3 Tb2' O28 -91.3(3) . .
O23 Tb3 Tb2' O30 96.9(5) . .
O23 Tb3 Tb2' O5W -44.1(6) . .
O23 Tb3 O11 Ge5 -6.0(4) . .
O23 Tb3 O11 Tb4 145.3(3) . .
O23 Tb3 O12 Ge6 18.5(3) . .
O23 Tb3 O12 Tb5 -153.9(3) . 3_667
O23 Tb3 O28 Tb2 72.3(3) . .
O23 Tb3 O28 Tb2' 68.8(3) . .
O23 Tb3 O28 C22 -92.7(8) . .
O23 Tb3 O30 Ge7 110.2(5) . .
O23 Tb3 O30 Tb2 -76.9(3) . .
O23 Tb3 O30 Tb2' -71.1(4) . .
O24 Tb2 Tb2' Ge7 116.8(13) . .
O24 Tb2 Tb2' Tb3 79.8(4) . .
O24 Tb2 Tb2' O18 154.6(4) . 3_667
O24 Tb2 Tb2' O25 -132.4(12) . .
O24 Tb2 Tb2' O28 69.4(6) . .
O24 Tb2 Tb2' O30 92.6(7) . .
O24 Tb2 Tb2' O5W -71.4(4) . .
O24 Tb2 N1 C23 -99.9(8) . .
O24 Tb2 N1 C27 92.8(10) . .
O24 Tb2 O25 Tb2 -143.9(3) . 3_566
O24 Tb2 O25 Tb2' 41.2(11) . .
O24 Tb2 O25 C21 -4(2) . .
O24 Tb2 O28 Tb3 -73.2(3) . .
O24 Tb2 O28 Tb2' -56.7(8) . .
O24 Tb2 O28 C22 90.9(8) . .
O24 Tb2 O30 Ge7 -96.2(4) . .
O24 Tb2 O30 Tb3 90.2(3) . .
O24 Tb2 O30 Tb2' -68.4(9) . .
O24 Tb2 O5W Tb2' 61.9(7) . .
O24 Tb2' O25 Tb2 -128.5(13) . .
O24 Tb2' O25 Tb2 -134.2(5) . 3_566
O24 Tb2' O25 C21 21.1(19) . .
O24 Tb2' O28 Tb2 112.2(9) . .
O24 Tb2' O28 Tb3 -83.8(3) . .
O24 Tb2' O28 C22 72.8(10) . .
O24 Tb2' O30 Ge7 -103.6(4) . .
O24 Tb2' O30 Tb2 101.1(10) . .
O24 Tb2' O30 Tb3 77.5(4) . .
O24 Tb2' O5W Tb2 -106.3(7) . .
O25 Tb2 Tb2' Ge7 -106.0(12) 3_566 .
O25 Tb2 Tb2' Ge7 -110.8(18) . .
O25 Tb2 Tb2' Tb3 -147.8(10) . .
O25 Tb2 Tb2' Tb3 -143.0(2) 3_566 .
O25 Tb2 Tb2' O18 -73.0(9) . 3_667
O25 Tb2 Tb2' O18 -68.2(3) 3_566 3_667
O25 Tb2 Tb2' O24 132.4(12) . .
O25 Tb2 Tb2' O24 137.2(3) 3_566 .
O25 Tb2 Tb2' O25 4.8(12) 3_566 .
O25 Tb2 Tb2' O28 -158.2(7) . .
O25 Tb2 Tb2' O28 -153.4(6) 3_566 .
O25 Tb2 Tb2' O30 -135.0(15) . .
O25 Tb2 Tb2' O30 -130.2(6) 3_566 .
O25 Tb2 Tb2' O5W 65.8(3) 3_566 .
O25 Tb2 Tb2' O5W 61.0(9) . .
O25 Tb2 N1 C23 122.3(8) 3_566 .
O25 Tb2 N1 C23 -177.4(7) . .
O25 Tb2 N1 C27 -45.0(10) 3_566 .
O25 Tb2 N1 C27 15.3(13) . .
O25 Tb2 O24 Tb2' -27.0(7) . .
O25 Tb2 O24 Tb2' -81.5(8) 3_566 .
O25 Tb2 O24 C18 -162.4(8) 3_566 .
O25 Tb2 O24 C18 -107.9(9) . .
O25 Tb2 O25 Tb2 0.001(1) 3_566 3_566
O25 Tb2 O25 Tb2' -174.9(12) 3_566 .
O25 Tb2 O25 C21 140(2) 3_566 .
O25 Tb2 O28 Tb3 11.8(7) . .
O25 Tb2 O28 Tb3 129.0(3) 3_566 .
O25 Tb2 O28 Tb2' 145.5(9) 3_566 .
O25 Tb2 O28 Tb2' 28.3(9) . .
O25 Tb2 O28 C22 -66.9(9) 3_566 .
O25 Tb2 O28 C22 175.9(8) . .
O25 Tb2 O30 Ge7 43.0(5) 3_566 .
O25 Tb2 O30 Ge7 -1.3(4) . .
O25 Tb2 O30 Tb3 -174.8(3) . .
O25 Tb2 O30 Tb3 -130.5(3) 3_566 .
O25 Tb2 O30 Tb2' 70.9(9) 3_566 .
O25 Tb2 O30 Tb2' 26.6(9) . .
O25 Tb2 O5W Tb2' -106.0(7) 3_566 .
O25 Tb2 O5W Tb2' -34.3(7) . .
O25 Tb2' O24 Tb2 142.3(10) . .
O25 Tb2' O24 C18 -108.4(9) . .
O25 Tb2' O28 Tb2 -95.2(19) . .
O25 Tb2' O28 Tb3 68.8(17) . .
O25 Tb2' O28 C22 -134.6(18) . .
O25 Tb2' O30 Ge7 8.5(5) . .
O25 Tb2' O30 Tb2 -146.8(11) . .
O25 Tb2' O30 Tb3 -170.5(4) . .
O25 Tb2' O5W Tb2 136.9(8) . .
O26 Tb2 Tb2' Ge7 -84.7(16) 3_566 .
O26 Tb2 Tb2' Tb3 -121.7(11) 3_566 .
O26 Tb2 Tb2' O18 -46.9(12) 3_566 3_667
O26 Tb2 Tb2' O24 158.6(9) 3_566 .
O26 Tb2 Tb2' O25 26(2) 3_566 .
O26 Tb2 Tb2' O28 -132.0(15) 3_566 .
O26 Tb2 Tb2' O30 -108.9(11) 3_566 .
O26 Tb2 Tb2' O5W 87.2(12) 3_566 .
O26 Tb2 N1 C23 87.9(8) 3_566 .
O26 Tb2 N1 C27 -79.4(10) 3_566 .
O26 Tb2 O24 Tb2' -160.6(8) 3_566 .
O26 Tb2 O24 C18 118.5(9) 3_566 .
O26 Tb2 O25 Tb2 9.4(4) 3_566 3_566
O26 Tb2 O25 Tb2' -165.6(12) 3_566 .
O26 Tb2 O25 C21 149(2) 3_566 .
O26 Tb2 O28 Tb3 140.6(3) 3_566 .
O26 Tb2 O28 Tb2' 157.1(8) 3_566 .
O26 Tb2 O28 C22 -55.3(8) 3_566 .
O26 Tb2 O30 Ge7 107.2(4) 3_566 .
O26 Tb2 O30 Tb3 -66.4(4) 3_566 .
O26 Tb2 O30 Tb2' 135.0(10) 3_566 .
O26 Tb2 O5W Tb2' -148.6(7) 3_566 .
O27 Tb4 Tb5 Tb3 -163.4(12) . 3_667
O27 Tb4 Tb5 O7 112.7(13) . 3_667
O27 Tb4 Tb5 O9 -125.1(12) . .
O27 Tb4 Tb5 O10 -82.4(12) . .
O27 Tb4 Tb5 O12 158.2(12) . 3_667
O27 Tb4 Tb5 O13 76.7(12) . 3_667
O27 Tb4 Tb5 O20 -46.4(12) . .
O27 Tb4 Tb5 O31 -8.0(15) . 3_667
O27 Tb4 Tb5 O3W 14.8(12) . .
O27 Tb4 O10 Ge4 7.7(7) . .
O27 Tb4 O10 Tb5 166.7(3) . .
O27 Tb4 O11 Ge5 88.7(4) . .
O27 Tb4 O11 Tb3 -67.3(3) . .
O27 Tb4 O21 C15 39.2(11) . .
O27 C22 C23 N1 175.1(10) . .
O27 C22 C23 C24 -5.7(16) . .
O28 Tb2 Tb2' Ge7 47.3(15) . .
O28 Tb2 Tb2' Tb3 10.3(5) . .
O28 Tb2 Tb2' O18 85.1(5) . 3_667
O28 Tb2 Tb2' O24 -69.4(6) . .
O28 Tb2 Tb2' O25 158.2(7) . .
O28 Tb2 Tb2' O30 23.2(10) . .
O28 Tb2 Tb2' O5W -140.8(5) . .
O28 Tb2 N1 C23 -9.0(7) . .
O28 Tb2 N1 C27 -176.2(11) . .
O28 Tb2 O24 Tb2' 124.3(7) . .
O28 Tb2 O24 C18 43.4(9) . .
O28 Tb2 O25 Tb2 132.2(5) . 3_566
O28 Tb2 O25 Tb2' -42.8(13) . .
O28 Tb2 O25 C21 -88(2) . .
O28 Tb2 O30 Ge7 173.1(4) . .
O28 Tb2 O30 Tb3 -0.4(2) . .
O28 Tb2 O30 Tb2' -159.0(9) . .
O28 Tb2 O5W Tb2' 130.2(7) . .
O28 Tb3 Tb4 Ge2 91.30(17) . 3_667
O28 Tb3 Tb4 Ge5 -90.92(17) . .
O28 Tb3 Tb4 Tb5 -179.65(17) . .
O28 Tb3 Tb4 O7 142.8(2) . 3_667
O28 Tb3 Tb4 O8 105.6(3) . 3_667
O28 Tb3 Tb4 O10 -142.5(2) . .
O28 Tb3 Tb4 O11 -102.8(3) . .
O28 Tb3 Tb4 O15 66.8(2) . 3_667
O28 Tb3 Tb4 O21 -68.6(2) . .
O28 Tb3 Tb4 O27 -2.2(2) . .
O28 Tb3 Tb4 O4W 2.1(4) . .
O28 Tb3 Tb2' Ge7 -171.2(3) . .
O28 Tb3 Tb2' Tb2 -12.1(6) . .
O28 Tb3 Tb2' O18 -86.6(3) . 3_667
O28 Tb3 Tb2' O24 89.6(4) . .
O28 Tb3 Tb2' O25 -159.2(6) . .
O28 Tb3 Tb2' O30 -171.8(5) . .
O28 Tb3 Tb2' O5W 47.2(6) . .
O28 Tb3 O11 Ge5 -78.6(5) . .
O28 Tb3 O11 Tb4 72.6(3) . .
O28 Tb3 O12 Ge6 23.4(5) . .
O28 Tb3 O12 Tb5 -149.0(3) . 3_667
O28 Tb3 O23 C18 -71.4(10) . .
O28 Tb3 O30 Ge7 -172.5(5) . .
O28 Tb3 O30 Tb2 0.4(2) . .
O28 Tb3 O30 Tb2' 6.2(4) . .
O28 Tb2' O24 Tb2 -45.9(6) . .
O28 Tb2' O24 C18 63.5(9) . .
O28 Tb2' O25 Tb2 75.3(18) . 3_566
O28 Tb2' O25 Tb2 81.0(18) . .
O28 Tb2' O25 C21 -129.3(19) . .
O28 Tb2' O30 Ge7 173.4(4) . .
O28 Tb2' O30 Tb2 18.1(8) . .
O28 Tb2' O30 Tb3 -5.5(3) . .
O28 Tb2' O5W Tb2 -31.6(5) . .
O28 C22 C23 N1 -1.5(14) . .
O28 C22 C23 C24 177.7(11) . .
O29 Ge7 Tb2' Tb2 74.7(14) . .
O29 Ge7 Tb2' Tb3 116.1(3) . .
O29 Ge7 Tb2' O18 37.7(4) . 3_667
O29 Ge7 Tb2' O24 -166.6(4) . .
O29 Ge7 Tb2' O25 -54.1(5) . .
O29 Ge7 Tb2' O28 110.2(4) . .
O29 Ge7 Tb2' O30 116.8(5) . .
O29 Ge7 Tb2' O5W -93.6(5) . .
O29 Ge7 O30 Tb2 -66.4(5) . .
O29 Ge7 O30 Tb3 105.5(5) . .
O29 Ge7 O30 Tb2' -73.3(5) . .
O29 Ge7 O31 Tb5 -127.3(7) . 3_667
O29 Ge7 C19 C20 48.5(14) . .
O30 Ge7 Tb2' Tb2 -42.1(13) . .
O30 Ge7 Tb2' Tb3 -0.6(4) . .
O30 Ge7 Tb2' O18 -79.1(4) . 3_667
O30 Ge7 Tb2' O24 76.6(5) . .
O30 Ge7 Tb2' O25 -170.8(6) . .
O30 Ge7 Tb2' O28 -6.6(4) . .
O30 Ge7 Tb2' O5W 149.6(7) . .
O30 Ge7 O31 Tb5 -9.7(7) . 3_667
O30 Ge7 C19 C20 -82.7(14) . .
O30 Tb2 Tb2' Ge7 24.2(7) . .
O30 Tb2 Tb2' Tb3 -12.8(6) . .
O30 Tb2 Tb2' O18 62.0(7) . 3_667
O30 Tb2 Tb2' O24 -92.6(7) . .
O30 Tb2 Tb2' O25 135.0(15) . .
O30 Tb2 Tb2' O28 -23.2(10) . .
O30 Tb2 Tb2' O5W -164.0(7) . .
O30 Tb2 N1 C23 -42.3(9) . .
O30 Tb2 N1 C27 150.5(9) . .
O30 Tb2 O24 Tb2' 48.4(7) . .
O30 Tb2 O24 C18 -32.5(9) . .
O30 Tb2 O25 Tb2 143.5(4) . 3_566
O30 Tb2 O25 Tb2' -31.4(11) . .
O30 Tb2 O25 C21 -77(2) . .
O30 Tb2 O28 Tb3 0.4(2) . .
O30 Tb2 O28 Tb2' 16.9(8) . .
O30 Tb2 O28 C22 164.5(8) . .
O30 Tb2 O5W Tb2' 15.8(7) . .
O30 Tb3 Tb4 Ge2 94.3(3) . 3_667
O30 Tb3 Tb4 Ge5 -88.0(3) . .
O30 Tb3 Tb4 Tb5 -176.7(3) . .
O30 Tb3 Tb4 O7 145.8(4) . 3_667
O30 Tb3 Tb4 O8 108.5(4) . 3_667
O30 Tb3 Tb4 O10 -139.5(4) . .
O30 Tb3 Tb4 O11 -99.9(4) . .
O30 Tb3 Tb4 O15 69.7(4) . 3_667
O30 Tb3 Tb4 O21 -65.7(4) . .
O30 Tb3 Tb4 O27 0.8(4) . .
O30 Tb3 Tb4 O4W 5.1(5) . .
O30 Tb3 Tb2' Ge7 0.6(4) . .
O30 Tb3 Tb2' Tb2 159.7(9) . .
O30 Tb3 Tb2' O18 85.2(5) . 3_667
O30 Tb3 Tb2' O24 -98.5(5) . .
O30 Tb3 Tb2' O25 12.6(5) . .
O30 Tb3 Tb2' O28 171.8(5) . .
O30 Tb3 Tb2' O5W -140.9(8) . .
O30 Tb3 O11 Ge5 -16.3(7) . .
O30 Tb3 O11 Tb4 135.0(3) . .
O30 Tb3 O12 Ge6 86.5(3) . .
O30 Tb3 O12 Tb5 -85.9(3) . 3_667
O30 Tb3 O23 C18 7.7(10) . .
O30 Tb3 O28 Tb2 -0.4(2) . .
O30 Tb3 O28 Tb2' -3.9(2) . .
O30 Tb3 O28 C22 -165.4(8) . .
O30 Tb2' O24 Tb2 -120.2(8) . .
O30 Tb2' O24 C18 -10.8(9) . .
O30 Tb2' O25 Tb2 141.9(13) . .
O30 Tb2' O25 Tb2 136.2(4) . 3_566
O30 Tb2' O25 C21 -68.4(17) . .
O30 Tb2' O28 Tb2 -159.3(10) . .
O30 Tb2' O28 Tb3 4.7(3) . .
O30 Tb2' O28 C22 161.3(10) . .
O30 Tb2' O5W Tb2 -138.5(17) . .
O31 Ge7 Tb2' Tb2 -44.6(16) . .
O31 Ge7 Tb2' Tb3 -3.2(6) . .
O31 Ge7 Tb2' O18 -81.7(6) . 3_667
O31 Ge7 Tb2' O24 74.0(6) . .
O31 Ge7 Tb2' O25 -173.4(6) . .
O31 Ge7 Tb2' O28 -9.1(6) . .
O31 Ge7 Tb2' O30 -2.6(7) . .
O31 Ge7 Tb2' O5W 147.0(6) . .
O31 Ge7 O30 Tb2 -174.6(4) . .
O31 Ge7 O30 Tb3 -2.7(6) . .
O31 Ge7 O30 Tb2' 178.5(4) . .
O31 Ge7 C19 C20 155.1(13) . .
O31 Tb5 O9 Ge3 -87.2(5) 3_667 .
O31 Tb5 O9 Tb3 78.5(3) 3_667 3_667
O31 Tb5 O10 Ge4 -1.3(6) 3_667 .
O31 Tb5 O10 Tb4 -162.8(3) 3_667 .
O31 Tb5 O20 C12 -78(2) 3_667 .
O1W Tb1 O1 Ge1 69.7(3) . .
O1W Tb1 O1 Ge2 -67.2(3) . .
O1W Tb1 O2 Ge2 68.8(3) . .
O1W Tb1 O2 Ge3 -69.1(3) . .
O1W Tb1 O3 Ge3 67.9(3) . .
O1W Tb1 O3 Ge4 -67.1(3) . .
O1W Tb1 O4 Ge4 67.4(3) . .
O1W Tb1 O4 Ge5 -69.5(3) . .
O1W Tb1 O5 Ge5 68.2(3) . .
O1W Tb1 O5 Ge6 -70.4(3) . .
O1W Tb1 O6 Ge1 -67.9(3) . .
O1W Tb1 O6 Ge6 70.7(3) . .
O2W Tb1 O1 Ge1 -79.3(4) . .
O2W Tb1 O1 Ge2 143.9(4) . .
O2W Tb1 O2 Ge2 -73.0(4) . .
O2W Tb1 O2 Ge3 149.1(3) . .
O2W Tb1 O3 Ge3 -107.7(6) . .
O2W Tb1 O3 Ge4 117.3(6) . .
O2W Tb1 O4 Ge4 -148.6(3) . .
O2W Tb1 O4 Ge5 74.5(4) . .
O2W Tb1 O5 Ge5 -145.6(4) . .
O2W Tb1 O5 Ge6 75.7(4) . .
O2W Tb1 O6 Ge1 109.5(5) . .
O2W Tb1 O6 Ge6 -111.9(5) . .
O3W Tb5 O9 Ge3 -0.1(7) . .
O3W Tb5 O9 Tb3 165.6(4) . 3_667
O3W Tb5 O10 Ge4 88.4(4) . .
O3W Tb5 O10 Tb4 -73.0(3) . .
O3W Tb5 O20 C12 31(2) . .
O4W Tb4 Tb5 Tb3 178.87(19) . 3_667
O4W Tb4 Tb5 O7 94.9(3) . 3_667
O4W Tb4 Tb5 O9 -142.9(3) . .
O4W Tb4 Tb5 O10 -100.1(3) . .
O4W Tb4 Tb5 O12 140.5(2) . 3_667
O4W Tb4 Tb5 O13 59.0(3) . 3_667
O4W Tb4 Tb5 O20 -64.1(3) . .
O4W Tb4 Tb5 O31 -25.8(9) . 3_667
O4W Tb4 Tb5 O3W -3.0(3) . .
O4W Tb4 O10 Ge4 -76.5(5) . .
O4W Tb4 O10 Tb5 82.6(3) . .
O4W Tb4 O11 Ge5 29.6(6) . .
O4W Tb4 O11 Tb3 -126.4(3) . .
O4W Tb4 O21 C15 -46.7(11) . .
O4W Tb4 O27 C22 172.0(12) . .
O5W Tb2 Tb2' Ge7 -171.8(12) . .
O5W Tb2 Tb2' Tb3 151.2(2) . .
O5W Tb2 Tb2' O18 -134.0(2) . 3_667
O5W Tb2 Tb2' O24 71.4(4) . .
O5W Tb2 Tb2' O25 -61.0(9) . .
O5W Tb2 Tb2' O28 140.8(5) . .
O5W Tb2 Tb2' O30 164.0(7) . .
O5W Tb2 N1 C23 -175.2(8) . .
O5W Tb2 N1 C27 17.5(10) . .
O5W Tb2 O24 Tb2' -98.4(7) . .
O5W Tb2 O24 C18 -179.2(9) . .
O5W Tb2 O25 Tb2 -71.6(3) . 3_566
O5W Tb2 O25 Tb2' 113.4(12) . .
O5W Tb2 O25 C21 68(2) . .
O5W Tb2 O28 Tb3 -136.3(3) . .
O5W Tb2 O28 Tb2' -119.8(9) . .
O5W Tb2 O28 C22 27.8(9) . .
O5W Tb2 O30 Ge7 -50.1(5) . .
O5W Tb2 O30 Tb3 136.3(3) . .
O5W Tb2 O30 Tb2' -22.3(10) . .
O5W Tb2' O24 Tb2 70.9(7) . .
O5W Tb2' O24 C18 -179.8(9) . .
O5W Tb2' O25 Tb2 -59.3(11) . .
O5W Tb2' O25 Tb2 -65.0(5) . 3_566
O5W Tb2' O25 C21 90.3(17) . .
O5W Tb2' O28 Tb2 41.7(7) . .
O5W Tb2' O28 Tb3 -154.3(3) . .
O5W Tb2' O28 C22 2.3(11) . .
O5W Tb2' O30 Ge7 -72.4(13) . .
O5W Tb2' O30 Tb2 132.3(19) . .
O5W Tb2' O30 Tb3 108.6(12) . .
C1 Ge1 O1 Ge2 -102.2(6) . .
C1 Ge1 O1 Tb1 133.4(4) . .
C1 Ge1 O6 Ge6 111.9(6) . .
C1 Ge1 O6 Tb1 -133.1(3) . .
C1 Ge1 O7 Tb4 82.8(5) . 3_667
C1 Ge1 O7 Tb5 -83.0(5) . 3_667
C1 C2 C3 O13 43.2(14) . .
C1 C2 C3 O14 -141.6(11) . .
C4 Ge2 Tb1 Ge5 -173.0(4) . .
C4 Ge2 Tb1 Ge6 127.7(4) . .
C4 Ge2 Tb1 O1 82.7(5) . .
C4 Ge2 Tb1 O2 -72.6(5) . .
C4 Ge2 Tb1 O3 -95.5(4) . .
C4 Ge2 Tb1 O4 -129.6(4) . .
C4 Ge2 Tb1 O5 142.5(5) . .
C4 Ge2 Tb1 O6 107.0(4) . .
C4 Ge2 Tb1 O14 -26.2(5) . 4_576
C4 Ge2 Tb1 O1W -173.9(4) . .
C4 Ge2 Tb1 O2W 45.7(5) . .
C4 Ge2 O1 Ge1 107.4(5) . .
C4 Ge2 O1 Tb1 -127.5(4) . .
C4 Ge2 O2 Ge3 -98.6(5) . .
C4 Ge2 O2 Tb1 132.7(4) . .
C4 Ge2 O8 Tb3 65.2(6) . 3_667
C4 Ge2 O8 Tb4 -79.0(5) . 3_667
C4 C5 C6 O15 34.4(14) . .
C4 C5 C6 O16 -151.5(11) . .
C7 Ge3 O2 Ge2 104.3(5) . .
C7 Ge3 O2 Tb1 -129.1(4) . .
C7 Ge3 O3 Ge4 -116.8(6) . .
C7 Ge3 O3 Tb1 130.7(4) . .
C7 Ge3 O9 Tb3 -83.0(5) . 3_667
C7 Ge3 O9 Tb5 81.3(6) . .
C7 C8 C9 O17 42.7(13) . .
C7 C8 C9 O18 -135.8(10) . .
C10 Ge4 O3 Ge3 114.9(6) . .
C10 Ge4 O3 Tb1 -132.6(4) . .
C10 Ge4 O4 Ge5 -102.8(6) . .
C10 Ge4 O4 Tb1 132.5(4) . .
C10 Ge4 O10 Tb4 77.9(6) . .
C10 Ge4 O10 Tb5 -79.5(5) . .
C10 C11 C12 O19 -160.7(14) . .
C10 C11 C12 O20 24.9(18) . .
C13 Ge5 Tb1 Ge2 -179.2(4) . .
C13 Ge5 Tb1 Ge6 -98.7(4) . .
C13 Ge5 Tb1 O1 -135.7(5) . .
C13 Ge5 Tb1 O2 137.3(5) . .
C13 Ge5 Tb1 O3 103.3(5) . .
C13 Ge5 Tb1 O4 80.6(5) . .
C13 Ge5 Tb1 O5 -75.8(5) . .
C13 Ge5 Tb1 O6 -100.0(5) . .
C13 Ge5 Tb1 O14 32.5(5) . 4_576
C13 Ge5 Tb1 O1W -178.3(5) . .
C13 Ge5 Tb1 O2W -39.1(5) . .
C13 Ge5 Tb4 Ge2 105.5(3) . 3_667
C13 Ge5 Tb4 Tb3 103.2(3) . .
C13 Ge5 Tb4 Tb5 -138.0(3) . .
C13 Ge5 Tb4 O7 -161.0(4) . 3_667
C13 Ge5 Tb4 O8 113.0(4) . 3_667
C13 Ge5 Tb4 O10 -128.3(4) . .
C13 Ge5 Tb4 O11 119.2(5) . .
C13 Ge5 Tb4 O15 52.9(5) . 3_667
C13 Ge5 Tb4 O21 -43.9(4) . .
C13 Ge5 Tb4 O27 33.9(4) . .
C13 Ge5 Tb4 O4W -39.9(4) . .
C13 Ge5 O4 Ge4 105.2(5) . .
C13 Ge5 O4 Tb1 -128.0(4) . .
C13 Ge5 O5 Ge6 -101.2(5) . .
C13 Ge5 O5 Tb1 130.2(4) . .
C13 Ge5 O11 Tb3 70.2(6) . .
C13 Ge5 O11 Tb4 -78.9(5) . .
C13 C14 C15 O21 30.3(14) . .
C13 C14 C15 O22 -151.8(11) . .
C16 Ge6 Tb1 Ge2 -123.2(4) . .
C16 Ge6 Tb1 Ge5 103.0(4) . .
C16 Ge6 Tb1 O1 -102.3(5) . .
C16 Ge6 Tb1 O2 -138.1(5) . .
C16 Ge6 Tb1 O3 135.5(5) . .
C16 Ge6 Tb1 O4 102.7(5) . .
C16 Ge6 Tb1 O5 78.7(5) . .
C16 Ge6 Tb1 O6 -79.5(5) . .
C16 Ge6 Tb1 O14 23.4(5) . 4_576
C16 Ge6 Tb1 O1W 179.9(5) . .
C16 Ge6 Tb1 O2W -21.0(5) . .
C16 Ge6 Tb3 Tb4 -136.5(4) . .
C16 Ge6 Tb3 Tb5 105.6(4) . 3_667
C16 Ge6 Tb3 Tb2' -7.6(4) . .
C16 Ge6 Tb3 O8 -166.0(4) . 3_667
C16 Ge6 Tb3 O9 109.8(4) . 3_667
C16 Ge6 Tb3 O11 -128.8(4) . .
C16 Ge6 Tb3 O12 110.7(5) . .
C16 Ge6 Tb3 O17 51.3(5) . 3_667
C16 Ge6 Tb3 O23 -44.3(4) . .
C16 Ge6 Tb3 O28 -53.2(4) . .
C16 Ge6 Tb3 O30 17.9(4) . .
C16 Ge6 O5 Ge5 106.7(5) . .
C16 Ge6 O5 Tb1 -126.3(4) . .
C16 Ge6 O6 Ge1 -115.8(6) . .
C16 Ge6 O6 Tb1 128.4(4) . .
C16 Ge6 O12 Tb3 -87.3(5) . .
C16 Ge6 O12 Tb5 82.8(6) . 3_667
C16 C17 C18 O23 39.2(13) . .
C16 C17 C18 O24 -142.2(10) . .
C19 Ge7 Tb2' Tb2 -173.0(14) . .
C19 Ge7 Tb2' Tb3 -131.6(4) . .
C19 Ge7 Tb2' O18 149.9(4) . 3_667
C19 Ge7 Tb2' O24 -54.4(5) . .
C19 Ge7 Tb2' O25 58.2(5) . .
C19 Ge7 Tb2' O28 -137.5(4) . .
C19 Ge7 Tb2' O30 -131.0(6) . .
C19 Ge7 Tb2' O5W 18.6(6) . .
C19 Ge7 O30 Tb2 64.2(6) . .
C19 Ge7 O30 Tb3 -123.9(5) . .
C19 Ge7 O30 Tb2' 57.3(6) . .
C19 Ge7 O31 Tb5 117.0(7) . 3_667
C19 C20 C21 O25 39(3) . .
C19 C20 C21 O26 -139.7(17) . .
C22 C23 C24 C25 -177.6(12) . .
C23 N1 C27 C26 1.2(19) . .
C23 C24 C25 C26 -1(2) . .
C24 C25 C26 C27 0(2) . .
C25 C26 C27 N1 0(2) . .
C27 N1 C23 C22 177.4(10) . .
C27 N1 C23 C24 -1.7(17) . .
